Biomaterials and Materials for Medicine: Innovations in Research, Devices, and Applications provides an application-orie
496 105 17MB
English Pages 384  Year 2021
Functionalized magnetic nanomaterials are used in data storage, biomedical, environmental, and heterogeneous catalysis a
169 96 53MB Read more
Mid-infrared Optoelectronics: Materials, Devices, and Applications addresses the new materials, devices and applications
692 89 25MB Read more
792 77 94MB Read more
Unlike conventional synchronous circuits, asynchronous circuits are not coordinated by a clocking signal, but instead us
366 73 8MB Read more
This book presents a state-of-the-art overview of the research and development in designing electrode and electrolyte ma
532 120 14MB Read more
Emerging 2D Materials and Devices for the Internet of Things: Information, Sensing and Energy Applications summarizes st
640 40 39MB Read more
This handbook brings together technical expertise, conceptual background, applications, and societal aspects of Industry
159 30 80MB Read more
Table of contents :
Table of Contents
Chapter 1 Cardiovascular Therapeutic Devices: Material and Fabrication Progress
1.2 Devices for Reestablishing Healthy Blood Circulation
1.2.1 Vena Cava Filter
22.214.171.124 Permanent Vena Cava Filter
126.96.36.199 Temporary Vena Cava Filter
188.8.131.52 Retrievable Vena Cava Filter
1.2.2 Embolization Devices
184.108.40.206 Non-absorbable Solid Particle Embolic Material
220.127.116.11 Absorbable Embolic Material
18.104.22.168 Mechanical Embolic Material
1.3 Devices for Implementing Revascularization
1.3.1 Vascular Stent
22.214.171.124 Major Drugs for DES Platforms
126.96.36.199 Optimization of DES Surface Coating and Structure
188.8.131.52 Trials of BRS
1.3.2 Drug-Coated Balloon
184.108.40.206 Approaches to Manipulate Tissue Uptake Rate of DCB Drug
220.127.116.11 Factors Relevant to Tissue Distribution and Resistance of DCB Drug
18.104.22.168 Alternation of DCB Drugs
1.3.3 Artificial Blood Vessel
22.214.171.124 Materials for Artificial Blood Vessel Fabrication
126.96.36.199 Surface Modification Technologies
188.8.131.52 Possibilities of Small Diameter Artificial Blood Vessel
1.4 Devices for Restoring Cardiac Hemodynamics
1.4.1 Artificial Heart Valves Replacement
184.108.40.206 Mechanical Valves
220.127.116.11 Tissue Valves
18.104.22.168 Tissue-Engineered Valves
1.4.2 Heart Function Recovery
22.214.171.124 Totally Artificial Heart
126.96.36.199 Ventricular Assist Devices (VADs)
Chapter 2 Vascular Patches: Past and Future, Problems, and Solutions
2.1 Animal Model
2.2 Patch Materials
2.3 Patch Healing After Implantation
2.4 Tissue-Engineered Vascular Patches
2.5 Complications of Patches
2.6 Future Research Directions
Chapter 3 Biomaterials for Fabricating Vascularized Scaffolds in Tissue Engineering
3.2 Biomaterials for Vascularization
3.2.1 Natural Polymers
188.8.131.52 Natural Proteins
184.108.40.206 Decellularized Extracellular Matrix
3.2.2 Synthetic Biomaterials
220.127.116.11 Poly(Ethylene Glycol)
18.104.22.168 Polyglycolide, Polylactide, and Their Copolymer Poly(Lactide-Co-Glycolide)
22.214.171.124 Poly(Glycerol Sebacate)
3.3 Fabrication Techniques for Engineering Vascularized Scaffolds
3.3.4 Particle Leaching
126.96.36.199 Inkjet Bioprinting
188.8.131.52 Extrusion Bioprinting
184.108.40.206 Laser-Assisted Bioprinting
220.127.116.11 Stereolithography Bioprinting
3.4 Modulating the Properties of Biomaterials
3.4.1 Modulating the Microstructures
3.4.2 Improve the Bioactivity of Scaffolds
3.4.3 Tuning the Biodegradation Property
3.4.4 Engineering Scaffolds with Rational Mechanical Properties
3.4.5 Gradients Fabrication of Tissue-Engineered Scaffolds
3.5 Current Limitation and Future Directions
Chapter 4 Biomaterials and Coatings for Artificial Hip Joints
4.1 Introduction: Background of Hip Joint Replacement
4.2 Normal Hip Joint and Artificial Hip Joint
4.2.1 Composition of Hip Joint
4.2.2 Causes of Implant Failure
4.3 Biomaterials for Artificial Hip Joints
4.3.1 Metallic Biomaterials for Artificial Hip Joint
18.104.22.168 Biocompatibility of Metal Implants
22.214.171.124 Mechanical Properties of Metal Implants
126.96.36.199 Tribocorrosion Properties of Metal Implants
4.3.2 Polymer Biomaterials for Artificial Hip Joints
188.8.131.52 Ultra-High-Molecular-Weight Polyethylene (UHMWPE)
184.108.40.206 Highly Cross-Linked Polyethylenes (HXLPEs)
4.3.3 Ceramic Biomaterials for Artificial Hip Joints
4.4 Classification for Artificial Hip Joints
4.4.1 Metal Femoral Heads Articulating Against Polyethylene Cups (MOP)
4.4.2 Metal Femoral Heads Articulating Against Metal Cups (MOM)
4.4.3 Ceramic Femoral Heads Articulating Against Polyethylene Cups (COP)
4.4.4 Ceramic Femoral Heads Articulating Against Ceramic Cups (COC)
4.5 Diamond-like Carbon (DLC) Coatings for Artificial Hip Joint
4.5.1 Classification and Deposition of DLC Coatings
4.5.2 Internal Stress of DLC Coatings
4.5.3 Adhesion of DLC Coatings
4.5.4 Biocompatibility of DLC Coatings
4.5.5 DLC-Coated Artificial Joint Friction Pairs
220.127.116.11 M-DLC/P Artificial Joint
18.104.22.168 DLC/M-P Artificial Joint
22.214.171.124 M-DLC/M Artificial Joint
126.96.36.199 DLC-DLC Artificial Joint
Chapter 5 Overview of Polymeric Biomaterials for Dental Applications
5.2 Endodontic Materials
5.2.1 Pulp Capping Materials
5.2.2 Root Canal Filling Materials
188.8.131.52 Solid Core Filling Points
184.108.40.206 Root Canal Sealer
5.2.3 Materials for Endodontic Regeneration
220.127.116.11 Naturally-Derived Polymeric Scaffolds
18.104.22.168 Synthetic Scaffolds
5.3 Materials for Periodontology
5.4 Materials for Impression
5.4.3 Polyvinyl Siloxanes
5.5 Materials for Prosthodontics
5.5.1 Restorative Material for Tooth Defect
22.214.171.124 Resin Composite
126.96.36.199 Adhesive Materials
5.5.2 Restorative Material for Dentition Defect
5.6 Materials for Orthodontics
5.7 Materials for Oral Implantology
Chapter 6 Recent Progress of Hydrogel in Skin Tissue Engineering
6.2 Complicated Structure and Functions of Skin
6.3 Types and Treatment of Skin Diseases
6.4 Wound Healing Mechanism
6.5 Skin Tissue Engineering
6.6 Structure and Properties of Hydrogels
6.7 Application of Natural Polymer Hydrogel Scaffold in Skin Tissue Engineering
6.8 Application of Synthetic Polymer Hydrogel Scaffold in Skin Tissue Engineering
6.9 Summary and Outlook
Chapter 7 3D Printing in Nerve Regeneration
7.1 Introduction: Nerve System
7.1.1 Central Nerve System
7.1.2 Peripheral Nerve System
7.2 Injury in Nerve System
7.3 Treatment of SCI and PNI Using Tissue Engineering Methods
7.3.1 Treatment of SCI
7.3.2 Treatment of PNI
7.4 Development of Nerve Implants: Preparation Methods
7.5 3D Printing Technology
7.6 Models for 3D Printing
7.7 Materials as “Bio-ink” for 3D Printing
7.8 Application of 3D Printing in Nerve Regeneration
7.9 Further Consideration beyond 3D Printing in Nerve Regeneration
7.10 Future Remarks
Conflicts of Interest
Chapter 8 Progress in Biomaterials for Application of Esophageal Stents
8.1 Introduction: Esophageal Cancer
8.1.1 Refractory Benign Esophageal Strictures (RBES)
8.2 Selection of Commercial Esophageal Stents
8.2.1 Self-Expandable Metal Stents (SEMS)
8.2.2 Self-Expandable Plastic Stents (SEPSs)
8.2.3 Polymer Degradable Stent
8.3 Improvement of the Esophageal Stent
8.3.1 Degradable Stent
8.3.2 Drug-Eluting Stents
8.3.3 Irradiation Stent
Chapter 9 High-Performance Materials for Targeted and Controlled Drug Delivery Systems
9.2 Biodegradable Polymers Used for Construction of Sustained/Controlled Drug Delivery Systems
9.2.1 Natural and Synthetic Biomaterials for controlled-release DDS
188.8.131.52 Synthetic Polymers
184.108.40.206 Natural Biomaterials
9.2.2 Formulation of Different Types of Controlled-Release Drug Delivery Systems
220.127.116.11 Sustained-Release Matrix Tablets
18.104.22.168 Biomaterials Used for Bioadhesive Drug Delivery System
22.214.171.124 Biomaterials Used for Membrane-Controlled Sustained-Release Preparation
9.2.3 Problems and Solutions
126.96.36.199 How to Eliminate Sudden Release of Drug from the Carriers?
188.8.131.52 Long Circulating Properties of DDS
184.108.40.206 How to Improve Controlled-Release Performance by Bioadhesion Polymers?
9.3 Application of Biomaterials in Targeted Drug Delivery System
9.3.1 Biomaterials Utilized for Different Targeting Mechanism
220.127.116.11 Biophysical Drug Targeting
18.104.22.168 Physical and Mechanical Targeting
22.214.171.124 Biochemical Targeting
126.96.36.199 Bioimmune Targeting
9.3.2 Different Types of Carriers
9.4 Future Perspectives
Chapter 10 Wearable/Attachable Sensors and Biosensors
10.2 Materials for Biosensor Devices
10.2.1 Wearable Substrates
10.2.2 Conducting Electrodes
10.2.3 Sensing Materials
10.3 Physical Biosensors
10.3.1 Working Principles of Physical Biosensors
10.3.1.1 Piezoelectricity-Based Sensors
10.3.1.2 Piezoresistivity-Based Sensor
10.3.1.3 Capacitance-Based Sensor
10.3.3 Heart Rate
10.3.4 Respiratory Rate
10.3.5 Blood Pressure
10.4 Chemical Biosensors
10.4.1 Working Principles of Chemical Sensors
10.5 Conclusion and Perspectives
Chapter 11 Micro/Nanobiomaterials
11.2 Micropattern in Biomaterial
11.3 Nanomedicine in Biomaterial
11.4 Micro/Nanobiodevices in Biomaterial
Chapter 12 Bioinspired Design for Medical Applications
12.2 Physical and Chemical Properties of Biomaterials
12.2.1 Biomaterial Topography
12.2.2 Biomaterial Chemistry
12.2.3 Biomaterial Wettability
12.3 Biomaterial Functionalization
12.3.1 Bioinspired Design for Osteointegration
188.8.131.52 Micro/Nanostructure Surface Design
12.3.2 Bioinspired Design for Blood Compatibility
184.108.40.206 Biomolecular Coating Design
220.127.116.11 Superhydrophobic Surface Design
18.104.22.168 Liquid Interface Design
12.3.3 Bioinspired Design to Enhance Antibacterial Properties
22.214.171.124 Antibacterial Coatings Design
12.3.4 Corrosion Resistance
Chapter 13 Modeling and Simulation of Biomaterials
13.2 Density Functional Theory
13.2.1 Schrödinger Equation of Many-Body System
13.2.2 Born–Oppenheimer Approximation
13.2.3 Hartree–Fock Approximation
13.2.4 Hohenberg–Kohn Theorem and Kohn-Sham Equation
13.2.5 Correlation Exchange Functional
13.3 Molecular Dynamics
13.3.1 The Process of MD Simulations
13.3.2 Force Field of MD Simulations
13.3.3 Molecular Dynamics Algorithm
126.96.36.199 Solving the Equation of Motion
188.8.131.52 Periodic Boundary Conditions of MD Simulations
184.108.40.206 Ensemble of MD Simulations
13.3.4 Enhanced Sampling Methods
220.127.116.11 Parallel Tempering
18.104.22.168 Simulated Annealing
22.214.171.124 Umbrella Sampling
13.4 Monte Carlo Method
Biomaterials and Materials for Medicine
Emerging Materials and Technologies Series Editor: Boris I. Kharissov Recycled Ceramics in Sustainable Concrete: Properties and Performance Kwok Wei Shah and Ghasan Fahim Huseien
Photo-Electrochemical Ammonia Synthesis: Nanocatalyst Discovery, Reactor Design, and Advanced Spectroscopy Mohammadreza Nazemi and Mostafa A. El-Sayed
Fire-Resistant Paper: Materials, Technologies, and Applications Ying-Jie Zhu
Sensors for Stretchable Electronics in Nanotechnology Kaushik Pal
Polymer-Based Composites: Design, Manufacturing, and Applications V. Arumugaprabu, R. Deepak Joel Johnson, M. Uthayakumar, and P. Sivaranjana
Nanomaterials in Bionanotechnology: Fundamentals and Applications Ravindra Pratap Singh and Kshitij RB Singh
Biomaterials and Materials for Medicine: Innovations in Research, Devices, and Applications Jingan Li
Advanced Materials and Technologies for Wastewater Treatment Sreedevi Upadhyayula and Amita Chaudhary
Biomaterials and Materials for Medicine Innovations in Research, Devices, and Applications
First edition published 2022 by CRC Press 6000 Broken Sound Parkway NW, Suite 300, Boca Raton, FL 33487-2742 and by CRC Press 2 Park Square, Milton Park, Abingdon, Oxon, OX14 4RN © 2022 Taylor & Francis Group, LLC CRC Press is an imprint of Taylor & Francis Group, LLC Reasonable efforts have been made to publish reliable data and information, but the author and publisher cannot assume responsibility for the validity of all materials or the consequences of their use. The authors and publishers have attempted to trace the copyright holders of all material reproduced in this publication and apologize to copyright holders if permission to publish in this form has not been obtained. If any copyright material has not been acknowledged please write and let us know so we may rectify in any future reprint. Except as permitted under U.S. Copyright Law, no part of this book may be reprinted, reproduced, transmitted, or utilized in any form by any electronic, mechanical, or other means, now known or hereafter invented, including photocopying, microfilming, and recording, or in any information storage or retrieval system, without written permission from the publishers. For permission to photocopy or use material electronically from this work, access www.copyright.com or contact the Copyright Clearance Center, Inc. (CCC), 222 Rosewood Drive, Danvers, MA 01923, 978750-8400. For works that are not available on CCC please contact [email protected] Trademark notice: Product or corporate names may be trademarks or registered trademarks and are used only for identification and explanation without intent to infringe. ISBN: 978-0-367-75321-4 (hbk) ISBN: 978-0-367-75323-8 (pbk) ISBN: 978-1-003-16198-1 (ebk) DOI: 10.1201/9781003161981 Typeset in Times by codeMantra
Contents Preface.......................................................................................................................ix Foreword....................................................................................................................xi Editor...................................................................................................................... xiii Contributors.............................................................................................................. xv Chapter 1 Cardiovascular Therapeutic Devices: Material and Fabrication Progress................................................................................................. 1 Xiao Luo, Dan Zou, and Li Li Chapter 2 Vascular Patches: Past and Future, Problems, and Solutions.............. 35 Hualong Bai, Yanhua Xu, Hao He, Xin Li, Chang Shu, Jingan Li, Quancheng Kan, and Alan Dardik Chapter 3 Biomaterials for Fabricating Vascularized Scaffolds in Tissue Engineering.......................................................................... 49 Yonghong Fan, Yinhua Qin, Xinxin Li, Yuhao Wang, Youqian Xu, and Chuhong Zhu Chapter 4 Biomaterials and Coatings for Artificial Hip Joints.......................... 105 Y. Ren Chapter 5 Overview of Polymeric Biomaterials for Dental Applications......... 145 Zichen Wu, Xiaoxuan Lu, Xiaowei Wang, Xiangyang Li, and Jialong Chen Chapter 6 Recent Progress of Hydrogel in Skin Tissue Engineering................ 177 Kun Zhang, Shuaimeng Guan, Longlong Cui, Jiankang Li, Jiaheng Liang, and Jingjing Su Chapter 7 3D Printing in Nerve Regeneration................................................... 211 Guicai Li and Liling Zhang Chapter 8 Progress in Biomaterials for Application of Esophageal Stents....... 233 Yachen Hou, Jingan Li, Aqeela Yasin, and Mujiahid Iqbal
Chapter 9 High-Performance Materials for Targeted and Controlled Drug Delivery Systems..................................................................... 257 Jinjie Zhang Chapter 10 Wearable/Attachable Sensors and Biosensors................................... 285 Jingwen Li, Haiyang Liu, and Yifeng Lei Chapter 11 Micro/Nanobiomaterials...................................................................307 Shuo Wang Chapter 12 Bioinspired Design for Medical Applications................................... 319 Feng Wu Chapter 13 Modeling and Simulation of Biomaterials........................................ 329 Zhe Fang, Yu Zhao, and Hongyan Wang Index....................................................................................................................... 351
Preface Many monographs on biomaterials have been published in recent years, which introduce the development of biomaterials from various aspects. However, biomaterials is a cutting-edge dynamic discipline. Therefore, in this book, new knowledge, technology, and concept of biomaterials worldwide, especially in developing countries, are summarized. Invited by CRC Press/Taylor & Francis’s Series Editor, Prof. Boris I. Kharissov, we, together with young scientists from 13 research groups, wrote this book entitled “Biomaterials and Materials for Medicine: Innovations in Research, Devices, and Applications” to join the Emerging Materials and Technologies Book Series. This book is application-oriented, covering nine research directions of biomaterials and medical materials, and is divided into 13 chapters. The first three chapters mainly introduce the research of vascular biomaterials, including the latest research on cardiovascular therapeutic devices, vascular patches, and biomaterials for vascular tissue engineering. Chapters 4 and 5 describe the research regarding orthopedic biomaterials in detail, including joint materials and dental materials. Chapter 6 focusses on recent research hotspots about skin tissue engineering biomaterials. Chapter 7 introduces the related research of nerve tissue engineering materials, including central nerve repair materials and peripheral nerve repair materials. Chapter 8 introduces non-mainstream biomaterials, which are special stent materials for palliative treatment of esophageal cancer and related technologies of surface modification. These design concepts and emerging technologies can also provide reference for other lumen interventions such as biliary tract and airway. Many biomaterials and related designs display high performance in drug targeting and controlled release, which will be elaborated in Chapter 9. Wearable biomedical devices is a new research field, thus its research progress is interpreted by an authoritative expert, Associate Professor Yifeng Lei from Wuhan University in Chapter 10. Micronscale and nanoscale biomaterials have been demonstrated to have a series of functions related to scale, which is discussed Chapter 11. Dr. Shuo Wang from the University of Tsukuba in Japan highlights the related research. Inspired by nature and learning from nature, the latest research progress of biomimetic materials in biomedical engineering is introduced in Chapter 12. Finally, the theoretical calculation and computer simulation of biomaterials, as a complementary discipline with physical experimental science, is elaborated in Chapter 13. Of course, the contents we introduce in this book cannot entirely cover the current knowledge of biomaterials and materials for medicine. To be practical, it is just a drop in the ocean for this discipline. However, it represents the knowledge of firstline scientists, especially the authors of this book, in their respective fields of understanding and academic achievement. In the future, we will invite more experts and scholars from around the world to introduce new knowledge and expound their views in this series of books.
Foreword At the invitation of Dr. Jingan Li, I am very pleased to write a foreword for the book “Biomaterials and Materials for Medicine: Innovations in Research, Devices, and Applications”. Biomaterials is one of the most important frontiers and interdisciplinary fields in the world today. Almost all implant devices, medical testing equipment, and drug carriers need the development of biomaterials. The field of biomaterials covers a wide range of disciplines in science and technology, including materials, biology, iatrology, pharmacy, physics, chemistry, and mathematics. In recent years, the development of biomaterial science and technology has been progressing rapidly. At the same time, many new and detailed branches in the field of biomaterials have emerged, and these latest research achievements and technologies have not been summarized yet. Hence, it is important to provide this information to a majority of readers in a simple and easy to understand fashion. The publication of the book “Biomaterials and Materials for Medicine: Innovations in Research, Devices, and Applications” is timely, almost concluding all directions of application-oriented biomaterials, such as cardiovascular materials, bone materials, nerve scaffold materials, scaffold materials for vascular tissue engineering, controlled drug release carrier materials, wearable medical device-related materials, and research on theoretical calculation of materials. The book is divided into 13 chapters, four of which are contributed by young scientists and teachers of Zhengzhou University. Zhengzhou University is a worldclass university under the Ministry of Education of the People’s Republic of China and the Henan provincial government. The disciplines of materials, chemistry, and medicine offered at the university have entered the world-class discipline construction sequence, while nine disciplines, including materials science and engineering, clinical medicine, chemistry, biology, history and culture of Central Plains, cancer prevention and treatment, resource processing and efficient utilization, engineering safety and disaster prevention, and morphology of consciousness and social governance, were selected as the first phase of the construction project of advantageous characteristic disciplines in Henan Province. Zhengzhou University also has the largest number of students in China, about 72,600 (according to statistics published in 2019). Therefore, our aptitude for science and technology is not only reflected in senior experts, scholars, and professors but also our students’ desire for the latest knowledge and the most advanced technology. For Zhengzhou University, the publication of this book meets the needs of some disciplines to a certain extent, but it only meets the short-term needs of some disciplines. We welcome more books like this.
Finally, we are willing to work together with global peers to promote the rapid development of biomaterials and materials for medicine, and also wish outstanding young scientists continue on the road of science. Shao-kang Guan Zhengzhou University, China
Editor Dr. Jingan Li is a professor at Zhengzhou University, China, and his research fields include biomaterials and advanced functional materials. So far, he has published more than 70 academic papers in international academic journals as the first author or corresponding author, including ACS Applied Materials & Interface, Bioactive Materials, Acta Biomateralia, Carbohydrate Polymers, and Journal of Materials Science & Technology. He has served as the editorial board member of 12 journals, including Stem Cells International (Lead Guest Editor) and Smart Materials in Medicine, and is also the invited reviewer of more than 40 academic journals. Till now, he has been invited to attend more than 30 international academic conferences as plenary speaker, keynote speaker, invited speaker, organizing committee member, technical program committee, and session chair, and he was honored with “China-Korea Young Scientist Award” (2015) and “IAAM Fellow” (2020). For detailed information please see: https://www.researchgate.net/profile/ Jingan_Li2.
Contributors Hualong Bai Department of Vascular and Endovascular Surgery First Affiliated Hospital of Zhengzhou University Zhengzhou, China and Key Vascular Physiology and Applied Research Laboratory of Zhengzhou City Zhengzhou, China Jialong Chen Key Laboratory of Oral Diseases Research of Anhui Province, Stomatologic Hospital and College Anhui Medical University Hefei, China Longlong Cui School of Life Science Zhengzhou University Zhengzhou, China Alan Dardik The Vascular Biology and Therapeutics Program Yale School of Medicine New Haven, Connecticut and Departments of Surgery and of Cellular and Molecular Physiology Yale School of Medicine New Haven, Connecticut and Department of Surgery Yale School of Medicine New Haven, Connecticut
Yonghong Fan Department of Anatomy Third Military Medical University Chongqing, China Zhe Fang School of Materials and Chemical Engineering Zhongyuan University of Technology Zhengzhou, China Shuaimeng Guan School of Life Science Zhengzhou University Zhengzhou, China Hao He Department of Vascular Surgery, the Second Xiangya Hospital Central South University Changsha, China Yachen Hou School of Material Science and Engineering & Henan Key Laboratory of Advanced Magnesium Alloy & Key Laboratory of Materials Processing and Mold Technology (Ministry of Education) Zhengzhou University Zhengzhou, China Mujiahid Iqbal School of Material Science and Engineering & Henan Key Laboratory of Advanced Magnesium Alloy & Key Laboratory of Materials Processing and Mold Technology (Ministry of Education) Zhengzhou University Zhengzhou, China xv
Quancheng Kan Department of Pharmacy The First Affiliated Hospital of Zhengzhou University Zhengzhou, China and Henan Key Laboratory of Precision Clinical Pharmacy Zhengzhou University Zhengzhou, China Yifeng Lei School of Power and Mechanical Engineering & the Institute of Technological Science Wuhan University Wuhan, China Guicai Li University of Nantong University Nantong, China Jiankang Li School of Life Science Zhengzhou University Zhengzhou, China Jingan Li School of Material Science and Engineering & Henan Key Laboratory of Advanced Magnesium Alloy & Key Laboratory of Materials Processing and Mold Rechnology (Ministry of Education) Zhengzhou University Zhengzhou, China Jingwen Li School of Power and Mechanical Engineering & the Institute of Technological Science Wuhan University Wuhan, China
Li Li Key Laboratory for Advanced Technologies of Materials (Ministry of Education), School of Material Science and Engineering Southwest Jiaotong University Chengdu, China Xiangyang Li Key Laboratory of Oral Diseases Research of Anhui Province, Stomatologic Hospital and College Anhui Medical University Hefei, China Xin Li Department of Vascular Surgery, the Second Xiangya Hospital Central South University Changsha, China Xinxin Li Institute of Primate Traslational Medical Kunming University of Science and Technology Kunming, China Jiaheng Liang School of Life Science Zhengzhou University Zhengzhou, China Haiyang Liu School of Power and Mechanical Engineering & the Institute of Technological Science Wuhan University Wuhan, China Xiaoxuan Lu Key Laboratory of Oral Diseases Research of Anhui Province, Stomatologic Hospital and College Anhui Medical University Hefei, China
Xiao Luo Key Laboratory for Advanced Technologies of Materials, Ministry of Education, School of Material Science and Engineering Southwest Jiaotong University Chengdu, China Yinhua Qin Department of Anatomy Third Military Medical University Chongqing, China Y. Ren Department of Materials Science and Engineering Henan University of Technology Zhengzhou, China Chang Shu Department of Vascular Surgery, the Second Xiangya Hospital Central South University Changsha, China and Department of Vascular Surgery, Fuwai Hospital Chinese Academy of Medical Sciences and Peking Union Medical College Beijing, China Jingjing Su School of Life Science Zhengzhou University Zhengzhou, China Hongyan Wang School of Materials Science and Engineering Zhengzhou University Zhengzhou, China
Shuo Wang Graduate School of Science and Technology University of Tsukuba Tsukuba, Japan Xiaowei Wang Key Laboratory of Oral Diseases Research of Anhui Province, Stomatologic Hospital and College Anhui Medical University Hefei, China Yuhao Wang Department of Anatomy Third Military Medical University Chongqing, China Zichen Wu Key Laboratory of Oral Diseases Research of Anhui Province, Stomatologic Hospital and College Anhui Medical University Hefei, China Feng Wu College of Physics and New Energy Xuzhou University of Technology Xuzhou, China Yanhua Xu Department of Internal Medicine The First Affiliated Hospital of Zhengzhou University Zhengzhou, China Youqian Xu Department of Anatomy Third Military Medical University Chongqing, China
Aqeela Yasin School of Material Science and Engineering & Henan Key Laboratory of Advanced Magnesium Alloy & Key Laboratory of Materials Processing and Mold Technology (Ministry of Education) Zhengzhou University Zhengzhou, China Jinjie Zhang School of Pharmacy Zhengzhou University Zhengzhou, China Kun Zhang School of Life Science Zhengzhou University Zhengzhou, China Liling Zhang University of Nantong University Nantong, China
Yu Zhao School of Materials Science and Engineering Zhengzhou University Zhengzhou, China Chuhong Zhu Department of Anatomy Third Military Medical University Chongqing, China Dan Zou Key Laboratory for Advanced Technologies of Materials (Ministry of Education), School of Material Science and Engineering Southwest Jiaotong University Chengdu, China
Cardiovascular Therapeutic Devices: Material and Fabrication Progress Xiao Luo, Dan Zou, and Li Li Southwest Jiaotong University
CONTENTS 1.1 Introduction....................................................................................................... 2 1.2 Devices for Reestablishing Healthy Blood Circulation..................................... 3 1.2.1 Vena Cava Filter.................................................................................... 3 126.96.36.199 Permanent Vena Cava Filter................................................... 4 188.8.131.52 Temporary Vena Cava Filter................................................... 5 184.108.40.206 Retrievable Vena Cava Filter.................................................. 6 1.2.2 Embolization Devices............................................................................ 7 220.127.116.11 Non-absorbable Solid Particle Embolic Material................... 7 18.104.22.168 Absorbable Embolic Material................................................. 7 22.214.171.124 Mechanical Embolic Material................................................8 1.3 Devices for Implementing Revascularization.................................................... 9 1.3.1 Vascular Stent...................................................................................... 10 126.96.36.199 Major Drugs for DES Platforms........................................... 10 188.8.131.52 Optimization of DES Surface Coating and Structure......................................................................... 11 184.108.40.206 Trials of BRS........................................................................ 11 1.3.2 Drug-Coated Balloon........................................................................... 12 220.127.116.11 Approaches to Manipulate Tissue Uptake Rate of DCB Drug................................................................ 12 18.104.22.168 Factors Relevant to Tissue Distribution and Resistance of DCB Drug...................................................... 14 22.214.171.124 Alternation of DCB Drugs.................................................... 14 1.3.3 Artificial Blood Vessel......................................................................... 15 126.96.36.199 Materials for Artificial Blood Vessel Fabrication................. 15 188.8.131.52 Surface Modification Technologies...................................... 16 184.108.40.206 Possibilities of Small Diameter Artificial Blood Vessel.......................................................... 17 DOI: 10.1201/9781003161981-1
Biomaterials and Materials for Medicine
1.4 Devices for Restoring Cardiac Hemodynamics.............................................. 18 1.4.1 Artificial Heart Valves Replacement................................................... 19 220.127.116.11 Mechanical Valves................................................................ 19 18.104.22.168 Tissue Valves........................................................................20 22.214.171.124 Tissue-Engineered Valves.....................................................20 1.4.2 Heart Function Recovery..................................................................... 21 126.96.36.199 Totally Artificial Heart......................................................... 22 188.8.131.52 Ventricular Assist Devices (VADs)...................................... 22 References................................................................................................................. 23
1.1 INTRODUCTION Peace and development are the main themes of the current era. In recent decades, the global social economy has developed rapidly, and the lifestyles of residents have been greatly improved. However, due to long-term unhealthy lifestyles or other congenital factors, the prevalence of cardiovascular diseases has increased significantly. According to a World Health Organization (WHO) survey, cardiovascular disease has become the leading cause of death in the global population, accounting for approximately 30% of the total deaths. Through blood circulation, the cardiovascular system provides the body with oxygen, transports nutrients, and transports metabolic waste. The stable operation of the cardiovascular system is an important guarantee for maintaining the health of the body. For patients suffering from severe heart diseases such as embolism, congenital heart defects, vascular stenosis, and heart failure (HF), effective treatments increasingly rely on therapeutic devices. During the last decades, biomaterial and medical communities have optimized and introduced various materials, as well as structure design and fabrication, approaches. These exploitations enhanced the therapeutic value of the devices, and the clinical success demonstrated great progress in reestablishing healthy blood circulation, implementing revascularization, and restoring cardiac hemodynamics. There are various methods of cardiovascular treatment devices to deal with different cardiovascular diseases. When dealing with problems such as thrombus blood, filters are selected to remove the blood clots. When faced with tissue lesions caused by abnormal blood vessels, embolization devices are used to create thrombus to block the diseased blood vessels to maintain normal and healthy blood circulation. In dealing with vascular diseases, such as atherosclerosis, vascular stents or drug balloons are used for interventional treatment. Artificial blood vessels are selected to replace diseased blood vessels. For heart hemodynamic disorders caused by abnormal heart function and other reasons, artificial heart valves or ventricular assist devices are used for improvement, and artificial hearts are used for replacement. In this chapter, the currently adopted/potential materials and methods that modulated the device properties of anti/pro-coagulation, anti-hyperplasia, and mechanical support are summarized and compared (Figure 1.1). The challenges cardiovascular therapeutic devices face and the opportunities that are emerging have also been identified.
Cardiovascular Therapeutic Devices
FIGURE 1.1 Scheme of medical devices applied to cardiovascular therapy. (a) reestablishing healthy body circulation, (b) implementing revascularization, and (c) restoring hemodynamics.
1.2 DEVICES FOR REESTABLISHING HEALTHY BLOOD CIRCULATION Maintaining and reestablishing healthy blood circulation is the primary goal of cardiovascular therapeutic devices. There are different vascular lesions due to different causes, and therapeutic devices encounter different and complex situations. Thrombus is the most common problem that needs to be dealt with. However, thrombus plays a role as a double-edged sword that cannot be arbitrarily defined as good or bad (as shown in Figure 1.2). Under certain conditions, a filter can be applied to blood clots; and under other conditions, an embolization device can be deployed to produce the thrombus to block the diseased blood vessels. Here, we introduce two typical cardiovascular therapeutic devices: vena cava filter (VCF) and embolization device, which were specifically used for thrombus to maintain and reestablish a healthy blood circulation.
1.2.1 Vena Cava Filter Pulmonary thromboembolism (PTE) is mainly caused by deep vein thrombosis (DVT). The main pathogenic mechanism is that abnormal blood coagulation in the deep vein cavity blocks the lumen and obstructs venous reflux by forming a thrombus. Thrombus passes through the vena cava and enters the pulmonary circulation through the heart. Then, large blood clots cause blockages and insufficient blood supply to the lung.
Biomaterials and Materials for Medicine
FIGURE 1.2 Thrombus for reestablishing healthy blood circulation.
There are some commonly used methods to prevent large thrombus from entering the pulmonary circulation, such as dissolving the thrombus, or using mechanical methods (e.g., VCF) to capture and artificially block its transportation route. The main principle is to place a filter in the blood vessel to catch thrombus, especially the relatively large thrombus, so that it cannot enter the heart and pulmonary circulation, thereby avoiding pulmonary embolism. The filter has the following characteristics: (1) the filter is usually designed as an umbrella- or a cone-shaped structure which can keep the blood pressure and flow changes without any risk even it has been filled. Meanwhile, blood flow parallel to the axis can inhibit the growth of the thrombus and break the thrombus, ensuring healthy blood circulation. (2) The conveying device has a small impact. (3) The filter can stably capture thrombus. Sometimes the source of thrombosis is the thrombus that has been captured. For life-threatening thrombus, the filter should have high and stable capture efficiency. Some filters allow a small amount of other small thrombi to pass, thereby avoiding the excessive accumulation of trapped thrombus and forming the filter embolism. According to clinical use, three types of VCF products are available in the market: permanent, temporary, and optional recyclable VCF. Their material and structural design directly affect the clinical effect. 184.108.40.206 Permanent Vena Cava Filter Metal VCF was first used clinically in the 1980s. Once this type of filter is placed, it cannot be removed without an operation. Representative products include Greenfield , Bird’s Nest , VenaTech LGM , Simon , and TrapEase .
1. Greenfield filter (GF) In 1973, Greenfield used an umbrella filter for clinical use. To date, GF is the most widely used filter available in the market and has become the reference structure for later filter designs. The first-generation GF filter adopts an overall tapered design, with a hook at the tail end of the strut, which is anchored on the vessel wall by the hook. It is placed by surgically incising the internal jugular vein or femoral vein. According to the geometric principle, more than 50% of the open section can
Cardiovascular Therapeutic Devices
still be maintained even if the thrombus fills 70% of the total length of the upper end of the cone. Therefore, the design of the GF ensures smooth blood circulation in the vena cava and captures clinically significant thrombi. 2. Bird’s Nest filter (BNF) In 1989, Cook Medical launched a new type of filter in the United States under the trade name Bird’s Nest filter (BNF). The stainless steel wire of this filter is randomly bent into a net-like structure, similar to a bird’s nest. 3. VenaTech LGM filter The first-generation LGM filter was designed and developed by LG Medical and was launched in France. The filter is made of a bio-/magnetic resonance imaging-compatible alloy Phynox (cobalt, chromium, iron, nickel, molybdenum) by stamping and spot welding. Six slightly curved alloy sheet bases are connected to a flat side, and the side rails are attached to the wall of the vena cava to provide stable support. 4. Simon nitinol filter (SNF) SNF is the first nickel-titanium alloy filter on the market. The alloy is composed of 53% nickel, 45% titanium, and 2% cobalt. This material is relatively soft at room temperature, but has thermal memory and can be restored to the original shape at body temperature. This alloy is corrosion-resistant, non-ferromagnetic, and stronger than steel, making it a suitable material for preparing VCFs. 5. TrapEase filter (TEF) This filter is integrated by laser cutting nickel-titanium alloy tubes. It has a symmetrical design. The two sides of the head and tail are mesh baskets which are connected by six side pillars. The six side pillars are arranged into six diamonds, so the TEF becomes the center. The double basket design provides two levels of thrombus capture. The proximal and distal ends of the six side struts have straight thorns to provide the anchoring function of the filter and prevents the filter from migrating to the head or caudal side. Compared with simple anticoagulation therapy, permanent VCF reduces the occurrence of fatal PTE; however, it increases the risk of recurrent DVT, embolism, and a series of complications over time, including filter perforation, shedding, migration, and filter breakage. These complications pose a permanent threat to the patient.
220.127.116.11 Temporary Vena Cava Filter To solve a series of clinical deficiencies of permanent VCFs, temporary VCFs were developed. After temporary VCFs are placed, the interventional device needs to be connected to the filter and placed outside the body. At the same time, urokinase is used for thrombolysis. Generally, thrombolysis is completed after 6 hours, and then the filter is retracted through the interventional device. A representative product is Tempofilter II  which consists of eight Phynox and needs to be connected to a restrictive catheter. Therefore, the filter itself does not need a fixed hook to ensure correct positioning. During the placement, the degree of endothelialization is minimized, which improves the safety of recovery. However, the biggest drawback of this method is that it is easy to cause infection at the puncture site, thrombus spread along
Biomaterials and Materials for Medicine
the interventional device, and filter displacement. At the same time, before the DVT is cured, the longest safe indwelling time of temporary VCFs in the body is often exceeded. Therefore, many temporary VCFs are replaced by permanent VCFs. 18.104.22.168 Retrievable Vena Cava Filter To solve the issues with permanent VCFs, while avoiding the shortcomings of temporary VCF with many side effects, a recovery hook for recovery was added to the VCF. After being placed in the body, it no longer needs to be connected to the interventional device. It can be permanently indwelled in the body according to the patient’s requirement. When the patient no longer needs the filter, it can be safely recycled. Representative products include Günther Tulip , Denali , Celect , and Crux Vena Cava .
1. Günther Tulip filter (GTF) GTF is made of Conichrome® (cobalt-chromium-nickel-molybdenumiron alloy). The configuration is similar to tulip petals, hence, the name tulip. Twelve alloy wires form a cone-shaped thrombus capture net with a recovery hook on the head. 2. Denali filter Denali adopts the integrated manufacturing process of laser cutting nitinol tube and polishes it. Structurally, the titanium anchor on the filter wire arm is removed and the end of the leg is redesigned. There is a diverging hook at the end of each leg. 3. Celect filter Celect evolved from Günther Tulip. In addition to the four pillars, there are eight independent arc support rods, which cannot only capture thrombus but also support the vena cava to improve the stability and self-control of the filter. 4. Crux Vena Cava filter This is a novel product. It has a symmetrical double helix structure. The relatively helical self-expanding nickel-titanium alloy is connected to form a filter frame. There are five tissue anchors on the frame to optimize fixation and limit penetration. In recent years, biodegradable polymer materials have become a research hotspot, especially in the field of interventional devices . Biodegradable materials have the characteristic of disappearing by themselves after they perform their functions, which cannot be achieved by traditional materials. This feature can meet the requirements of clinical use of VCF: VCF plays a role in filtering thrombus in the early stage of implantation; in the late stage it gradually degrades as thrombosis continues to decrease; and finally, it is completely absorbed and discharged from the body. The clinical use of degradable VCF is expected to eliminate a series of complications caused by the late stage of permanent VCF implantation; on the other hand, it is expected to eliminate the secondary trauma to patients caused by retrievable VCF. Compared with metal VCF, the structural design and mechanical properties of degradable VCF are challenging. With the development of medical materials, processing technology, and new structural design, biodegradable VCFs will be the next generation of VCF in the future.
Cardiovascular Therapeutic Devices
1.2.2 Embolization Devices In the clinical treatment of intracranial aneurysms, intravascular embolization is usually required. In this situation, we need an embolization device to produce the thrombus quickly to block the blood vessels. Usually, embolic agents are injected into the supply vessels of the diseased organs or the diseased blood vessels to block them and interrupt the blood supply to control bleeding, treat vascular diseases and tumors, and eliminate the function of diseased organs. Broadly, an embolization device includes different devices and materials which achieve embolization. The ideal embolization device needs to travel smoothly in the blood vessel and should have the following characteristics: (1) Good biocompatibility, non-toxic, and non-antigenic. (2) Easy to transmit through the catheter without sticking and blocking the tube. (3) Occlude blood vessels quickly and applicable to different calibers and different flows as needed. An embolization device can be classified as follows: (1) According to the nature of the material, it can be divided into three categories: inactive materials, self-materials, and radioactive particles. (2) According to physical properties, it can be divided into solid and liquid embolic materials. (3) According to the duration for vascular occlusion, it can be divided into short-term, medium-term, and long-term. (4) According to whether the material can be absorbed by the body, it can be divided into absorbable and non-absorbable embolic materials. 22.214.171.124 Non-absorbable Solid Particle Embolic Material 1. Polyvinyl alcohol (PVA) particles PVA particles are made of PVA and formaldehyde through cross-linking, drying, crushing, and sieving. They are non-water soluble, swellable, and when exposed to aqueous liquids, their volume increases by 20%. They have good biocompatibility and are not absorbed in the body. 2. Elastic microsphere Poly-hydroxyethyl methacrylate (PHEMA) microsphere: the advantage of elastic microspheres is that they can be compressed in diameter and are easy to transport. 3. Shape memory polymer materials When processed into thin strips at low temperature, the shape of memory polymer material becomes thicker and shorter at body temperature and can be used for embolization [12,13]. 126.96.36.199 Absorbable Embolic Material 1. Autologous blood clot An autologous blood clot is a short-term embolism, which is easy to obtain and easy to inject through a sterile and non-antigenic catheter. The disadvantage is that the time to occlude the blood vessel cannot be predicted. 2. Gelatin sponge Gelatin sponge is a hemostatic agent for surgical operation. It is a protein matrix sponge and can be absorbed by tissues. After the gelatin sponge blocks blood vessels, it acts as a net frame and can quickly form
Biomaterials and Materials for Medicine
a thrombus. It offers a non-permanent occlusion, which lasts from a few weeks to several months. 3. Microcollagen fiber hemostatic agent Microcollagen fibers, a derivative of cowhide collagen, are usually used to stop bleeding during surgery and are more effective than gelatin sponge. The advantage is that they can enter small arteries; however, they may cause extensive interruption of the collateral blood supply due to tissue ischemia infarction. 4. Alginate microspheres Sodium alginate microspheres have good biocompatibility, are nontoxic, non-antigenic, non-chemical, or offer immune effects after embolization. Moreover, non-toxic degradation of microspheres occurs within 3–6 months.
188.8.131.52 Mechanical Embolic Material 1. Microcoil According to material classification, microcoils can be divided into copper coil , tungsten coil , and platinum coil . I. Copper coil: Copper can be easily oxidized in the body, and it has been used in neonatal Galen vein aneurysms. II. Tungsten coil: Tungsten is less flexible than platinum, and the friction force in the micropipette are greater; however, it remains stable after placement. III. Platinum coil: Platinum has good impermeability to X-ray, which can be observed on the fluorescent screen. Because platinum is very soft, when the pressure in the lumen increases slightly, the coil can adapt to the shape and size of the aneurysm very well. According to the control method of the coil, it can be divided into a free coil, electrolytic detachable coil [17–19], mechanical detachable spiral coil [20–22], and hydrolysis detachable coil [23–26]. I. Free coil: There is no connection device between the free coil and the thruster. The thruster can only push the coil and cannot withdraw. Therefore, it is dangerous and limits its application. II. Electrolytic detachable coil: Guglielmi’s detachable coil is a representative electrolytic detachable coil. The connection between the thruster and the microcoil adopts microwelding technology. After the coil reaches the proper position, the pusher is connected to the positive electrode of the power supply and weak direct current is passed. The stainless steel surface which is not covered with the insulating layer between the platinum coil and the pusher is electrolyzed so that the coil can be released without pulling in the aneurysm. This feature can reduce the mistaken embolism caused by the coil entering the tumor-bearing artery. III. Mechanically detachable spiral coil: Its performance and effect are similar to the electrolytic detachable coil. The main difference is that the tungsten wire coil is released mechanically, and the coil can be pulled back or repositioned freely until the position is satisfied. At present, there are three different release devices, namely, clamp type, collar
Cardiovascular Therapeutic Devices
type, and internal locking type. The internal locking type has low friction in the microcatheter and has good stability during release, which is better than the other two types. IV. Hydrolysis detachable coil: The catheter is expanded by increasing the water pressure so that the release coil does not require an additional power supply, which is stable and reliable, and only requires two syringes. A new type of coil hydro coil is coated with a hydrogel layer. After being placed in the aneurysm, the hydrogel begins to expand and fills the aneurysm space. As the hydrogel expands, the blood promotes healing components (such as proteins) which are inhaled into the hydrogel to improve the healing rate. Matrix coil is coated with degradable polymer materials, which can block blood flow in the aneurysm, induce thrombosis, and improve the embolization effect. Coating on the surface of the microcoil to enhance the embolization function is an efficient way to improve the clinical application value, including constructing a ciliary surface, hydrogel surface, and procoagulant protein coatings [27–30], which can effectively improve the embolization effect, promote wound repair and healing, and reduce complications. 2. Detachable balloon There are two types of detachable balloons: latex balloon and silicone balloon. The balloon should be filled with a permanent filler during application and should be used in conjunction with the microcatheter. After the balloon enters the tumor and inflates, the catheter is gently pulled to release the balloon. At present, it is only clinically suitable for the embolization treatment of aneurysms of the basilar artery bifurcation of the skull base, ophthalmic aneurysms, occlusion tests, and internal carotid artery cavernous fistula. 3. Silk thread Silk thread is also a type of embolic material, which plays a role in the endovascular treatment of cerebral arteriovenous malformation. It can be emblazed alone or combined with α-n-butyl cyanoacrylate. With further understanding of the mechanism of different cardiovascular diseases, the design of the cardiovascular therapeutic device and the development of material science for maintaining and reestablishing healthy blood circulation is becoming more and more targeted, personalized, and multi-functional. Especially dealing with the complex situation caused by thrombus, a new generation of cardiovascular therapeutic device can not only solve the problem of blood circulation but also provide a bioactive surface to promote therapeutic recovery of the diseased area and achieve a better therapeutic effect.
1.3 DEVICES FOR IMPLEMENTING REVASCULARIZATION The blood supply chain is crucial for normal body function, and a supply failure leads to tissue or organ death. Possible causes include thrombosis, vascular occlusion, vessel damage, and gangrene. Medicine, intervention, and bypass therapies are available for different lesion severity. The lesion sites are either reopened or repaired
Biomaterials and Materials for Medicine
based on the existing blood vessel or are replaced by a new one. This section focuses on intervention and bypass therapies. Three major therapeutic devices for revascularization are discussed: vascular stent, drug-coated balloon, and artificial blood vessel.
1.3.1 Vascular Stent In 1977, a distensible balloon was inflated to reopen the narrowed vessel, which reduced 50% vascular stenosis, and the percutaneous transluminal coronary angioplasty (PTCA) strategy emerged . However, vascular elastic retraction reduced the efficacy. To prevent the retraction and provide long-term mechanical support, a vascular stent was accordingly developed, which brought a revolutionary change to vascular disease treatment. They are widely used for occlusive vessels (e.g., coronary artery, brain artery, renal artery, main aorta). Vascular stents have passed through three stages: bare-metal stent (BMS), drug-eluting stent (DES), and bioresorbable stent (BRS), and the performance of a stent platform depends on three important elements as shown in Figure 1.3. BMS (medical stainless steel, nitinol, cobalt, etc.) successfully overcame the vascular elastic retraction and dramatically reduced the second intervention rate; however, the thrombosis and in-stent restenosis issues gave way to DES . 184.108.40.206 Major Drugs for DES Platforms DES consists of a BMS-based metallic backbone, extra surface coating, and drug. Clinically used DES platforms include Xience-V (Abbott Vascular), Endeavor (Medtronic), Biomatrix (Biosensors), Promus element (Boston Scientific), and Cypher (Cordis) . By coating stents with drugs that prevent smooth muscle cell (SMC) proliferation, in-stent restenosis can be considerably attenuated. The major drugs
FIGURE 1.3 Vascular stents platform.
Cardiovascular Therapeutic Devices
loaded to DES are mTOR inhibitors (rapamycin (sirolimus), everolimus, zotarolimus, biolimus), calcineurin inhibitors (tacrolimus, pimecrolimus), taxans (paclitaxel), hormones (estradiol), cytotoxic antibiotics (actinomycin D), and combination with tested drugs (cerivastatin, batimastat, flavopiridol, probucol, carvedilol) . mTOR inhibitors showed a superior clinical effect compared to others, and the outcome of sirolimus was independent of the presence of polymer coating. Taxans also produced beneficial effect, notwithstanding that their cytotoxicity and narrow therapeutic wind brought severe side effects for peripheral artery disease such as thrombosis and inflammation . However, these beneficial drugs halt the growth of endothelial cells as well as neointimal tissue, and stent struts along with the remaining coating continually stimulate the vessel wall, hence, it prolongs the chronic inflammation and delays the reendothelialization process that is vital for preventing late/very late thrombosis and in-stent restenosis. 220.127.116.11 Optimization of DES Surface Coating and Structure To cope with these issues, varied surface coatings have been fabricated. Isolating coatings (titanium, carbon, silicon carbide, etc.) have been used to reduce the interaction between stent metal ions and blood proteins as thrombosis was originally thought to be induced by charge transfer from plasma protein to metal. Bioactive coatings (e.g., heparin, phosphorylcholine (PC), nitric oxide) were deployed to inhibit the coagulation process . Degradable coatings have also been introduced: poly(L-lactic acid-co-Glycolic acid) (PLGA), PLA, and poly(L-lactic acid) (PLLA) . However, all coatings must be tailored to the interfacial bonding property, fracture risk, and biocompatibility. Degradable coatings have to further balance the rate among drug-release profile, coating degradation, and stent reendothelialization. Stent structure has also been shown to be involved in these complications. Boston refined structure from 132 μm of Taxus express to 81 μm of Promus element, and the late lumen loss was reduced more than 50% . This is consistent with the finding that stent thickness is positively related to in-stent restenosis rate . Firehawk (Microport Medical) was lasered with one side grooves to carry drug coating, which reduced the stimulus to blood composition and provided a comparable late thrombosis rate with Xience . Nano plus (Lepu Medical) adopted nano/micropore to load drug, which thoroughly eliminated coating impacts . 18.104.22.168 Trials of BRS To pursue a “leaving nothing behind” concept, the stent platform should disappear after providing transient mechanical support. To this end, polymer and metallic BRS have been developed. Most polymer BRS adopted PLLA, Poly(D, L-lactic acid) (PDLLA), proprietary tyrocore desaminotyrosine poly-carbonate (PTD-PC) as stent backbone, either fabricated with the drug directly or coated with a degradable drug film. Approximately 34 prospective polymer BRS are currently under development (e.g., Igaki-Tamai (Kyoto Medical), Absorb 1.0/2.0(Abbott Vascular), DESolve, MeRes100 (Meril), Xinsorb (Huaan), Fortitude (Amaranth Medical), Art18AZ(ART), Ideal BioStent (Xenogenics)), wherein Abbott and Igaki-Tamai stent platforms have gained CE marks, respectively, for coronary intervention and peripheral arterial diseases [33,39]. However, in 2017, Abbott withdrew the stent from the market due to
Biomaterials and Materials for Medicine
a disappointing mid-term outcome such as elevated thrombosis rate, which raised concerns about the use of polymer BRS. Despite the uncertainty, the enthusiasm for metallic biodegradable stent continued. Metallic BRS deployed magnesium, iron, and zinc as stent backbone with a polymer drug coating (e.g., Dreams (Biotronik), Unity (QualiMed), IBS(LifeTech)) [33,40]. Zinc-based alloy provides a promising platform and has just started its journey for BRS application . Magmaris (DREAMS 2G) (PLLA and sirolimus) was upgraded from AMS-1, which is the only metallic BRS that has gained a CE mark so far. Through fining alloy composition, strut thickness, crown design, and adding/refreshing drug-polymer coating, Magmaris possesses similar mechanical properties to DES, a smaller strut-to-artery ratio to the Absorb, and a tailored degradation process. Ultimately, it attained a target lesion failure and target lesion revascularization within the DES ranges, which demonstrated a safe device in simple lesions [42–44]. Clinically, first-generation DES has been replaced by second and third-generation ones due to a high risk of late stent thromboses . However, BMS still benefits patients under some specific conditions such as big diameter vessel disease and patients with bleeding antithrombosis conflict. Though BRS is still in its infancy, it has a promising future . Among these three types of stent platforms, the average strut thickness of metallic non-biodegradable stents is smaller than that of polymeric ones; however, there is almost no difference in coating materials and drug choices among the three types of stents . Therefore, it can be concluded that on the premise of the same drug choice and target function, subsequent beneficial stent relies on newly introduced stent backbone material, structure design, and tailored coating to allow rapid reendothelialization and minimize the risk of late/very late thrombosis, in-stent restenosis, and in-stent neo-atherosclerosis.
1.3.2 Drug-Coated Balloon PTCA strategy has gone through a spiral development. Balloon’s role evolved from purely reopening the vessel wall, to assisting stent implantation, to reopening and treating the diseased vessel. Due to the side effects of in-stent restenosis, late thrombosis, and long-term anti-platelet therapy, a drug-coated balloon (DCB) was developed as a non-stent therapeutic approach to the concept of “leaving nothing behind” . DCB carried anti-proliferative drugs on the balloon surface and transferred them to the lesion sites by compressing the plaque, which reduced anti-platelet therapy duration as well as restenosis rate. 22.214.171.124 Approaches to Manipulate Tissue Uptake Rate of DCB Drug To achieve therapeutic efficacy during a short contact with the vessel wall, the carried drug should be rapidly taken by the tissue. Paclitaxel was the most deployed drug for DCB as the lipophilic drug transferred easier than the hydrophilic drug. Although a dose of 2–3 μg/mm2 was reported to successfully inhibit restenosis , most paclitaxel did not reach the lesion. Paclitaxel-coated drug balloon lost about 60%–80% of the drug, and only approximately 16% of the drug was transferred to the intima of target sites . To overcome low transfer and high wash-off rate, one solution is avoiding unnecessary contact between drug and blood flow. DIOR had manufactured
Cardiovascular Therapeutic Devices
FIGURE 1.4 Methods for manipulating tissue uptake rate of DCB drug. (a) Microporous balloon, (b) linear-micropatterned balloon, (c) microneedled balloon, (d) crystalline coating, (e) non-crystalline coating, (f) nano-encapsulation.
a porous balloon with multiple micropores on the surface, with the drug embedded inside (Figure 1.4a) . Another option is increasing the contact pressure. Balloon with micropatterned array has been found to have a higher contact pressure between the endothelium and balloon surface, delivering 2.3 times higher amount of drug to lesions (Figure 1.4b) . Different from micropore and arrays attaching to the tissue surface, taking the drug directly into the tissue is one step further. Microneedle with a diameter of approximately 140 μm has been reported to cross the endothelium barrier into the base media and even deep into the adventitia (Figure 1.4c) [51,52]. Another unique approach is double-balloon layers. It was manufactured into an inner drug layer and an outer drug-free layer, which carried two-fold drugs (6.8 ± 0.7 μg/ mm2) as normal and delivered similar amounts during each inflation . Yet, both microneedle and double layers resulted in heterogeneous drug distribution. In addition to balloon structures, tissue uptake rate can be manipulated by surface coating. Currently, based on coating structure, DCB has developed from heterogeneous crystalline coating, to homogeneous non-crystalline coating, to homogeneous encapsulated microcrystalline coating (Figure 1.4d–f) . The crystalline coating usually raises the particulate issue and may cause downstream embolization , which was deduced as a possibility of high mortality of PCB in a meta-analysis . Heterogeneous coating increased the chances of heterogeneous drug distribution in lesion sites, and a subtherapeutic dose afterward. From crystalline to non-/ microcrystalline, excipients were the most common component for balloon coating, which were introduced as a hydrophilic spacer to create a high-contact surface area at lesion sites , and were found to enhance drug migration more than 10-fold . Excipients for commercial DCB treating cardiovascular restenosis include urea (IN.
Biomaterials and Materials for Medicine
PACT, Medtronic), either polysorbate or sorbitol (Lutonix, Bard), shellac (Restore, Cardionovum), iopromide (Paccocath, Bayer AG), and butyryl trihexyl citrate (Pantera Lux, Biotronik AG) . However, different coating formulations generated drug particles of different sizes. For example, IN.PACT Admiral DCB possessed larger particles than Lutonix and Ranger [54,55], whether the particle size is related to a downstream embolization is not certain so far. With or without an excipient, polymers were also deployed as a matrix to carry drugs. Poly(ethylene oxide) was designed for a two-phase drug release: small amount of drug at inflation stage and therapeutic amount at treatment stage . However, a heterogeneity issue emerged on balloon surface after first-round inflation when being fabricated into double layers . Recently, the possibilities of nanoparticle delivery system have been valued to improve delivery efficacy. Along with coating components, several commonly employed coating methods emerged, including dipping, spraying, surface grafting, LBL, hydrogel coating, and microsyringe. Due to poor interaction, dip coating suffered from severe washoff rates [57,58]. Compared to dipping, precise microsyringe allowed higher coating uniformity, which significantly improved paclitaxel uptake at the proximal and distal sites, and enhanced the total tissue uptake by approximately 42% than heterogeneous coating . Although paclitaxel is the default drug for most DCB that is under investigation, the different delivery efficacies between conical urea and spherical shellac, between nanoparticle carriers of UPE and PLGA, and between acrylic and LBL electrostatic coating methods illustrated the critical role that balloon coating plays in drug transfer [57,60]. 126.96.36.199 Factors Relevant to Tissue Distribution and Resistance of DCB Drug Following tissue uptake, therapeutic efficacy requires prolonged drug persistence in the vessel wall. It has been reported that only 1% drug is taken up by tissue, and the restenosis inhibition ability of paclitaxel is dose-dependent, though lower-dose PCB generates fewer peri-strut fibrin deposits [35,55]. Therefore, a subtherapeutic level of the tissue-retained drug would not work well . Paclitaxel exists in three forms as amorphous solid, anhydrous crystals, and dihydrate crystals . Both anhydrous and dihydrate have a higher tissue retention rate, and among mixed forms, both microcrystalline coating and amorphous/dihydrate coating have a higher tissue retention rate. If lesions sites were premounted with stents, they can achieve a higher drug halflife of about 1.9 months . High-contact pressure between tissue and balloon may also enhance drug persistence by facilitating a deeper delivery, like a balloon with microarrays . Instead of drug-delivering amounts, drug penetration ability was a key factor for balloon coating, especially carriers, to achieve long drug persistence. 188.8.131.52 Alternation of DCB Drugs Attributed to advanced coating technologies, DCB drug tends to be upgraded from paclitaxel to limus drug (sirolimus and zotarolimus) [54,63]. Paclitaxel can diffuse into the vessel wall easily because it is highly lipophilic. However, its earlier application for stent coronary interventions caused side effects of either stent thrombosis at high concentration or inflammatory response at a lower dose . Furthermore, due to a higher rate of mortality caused by paclitaxel-coated balloon in femoropopliteal arteries, a hypothesis was recently concluded that paclitaxel may cause long-term
Cardiovascular Therapeutic Devices
focal toxicity, though the concentration of the wash-off drug in plasma was below level causing systemic toxicity. Following paclitaxel’s step, focus was given to sirolimus, a default stent-carried drug wide therapeutic window. However, poorer lipophilicity limited its delivery from balloon surface to vessel wall, and normal strategies for PCB drug transfer and retention did not suit SCB . A new microcrystalline and encapsulation approach was developed to improve this. Sirolimus was encapsulated in a lipophilic package with an excipient and transferred into the intima after 1 hour, media after 3 days, and adventitia after 7 days . In addition sirolimus, other less toxic drugs such as metacept-3 were also under investigation . In recent decades, both balloon structures and surface properties were renewed to implement a balloon-only strategy. It provided an alternative therapeutic method to stenting and presented favorable clinical results in indications of small vessel disease, de-novo coronary lesions, bifurcation lesions, patients at high bleeding risk , and neurovascular disease . Concerns of high wash-off rate, low tissue retention, elastic recoil, coronary dissection , and distal embolization  are expected to be resolved in the future.
1.3.3 Artificial Blood Vessel Artificial blood vessels are medical devices used to restore blood circulation in the settings of diseased or damaged arteries and veins or as hemodialysis fistula. An ideal artificial blood vessel requires good biocompatibility, especially hemocompatibility, suitable mechanical property, similar dynamics performance with host vessel, low immunogenicity, strong resistance to infection, and off-the-shelf availability . Both autogenous vessels and allografts are the primary choices for artificial blood vessels, but their sources are limited and a second injury is always problematic. To overcome these, in 1952, Voorhees introduced a groundbreaking device – permeable artificial blood vessel Vinylon “N” – which was successful in both dog and human tests . Since then, a variety of alternative grafts have been investigated in the past 60 years, including bioprosthetic, synthetic, and tissue-engineered grafts. 184.108.40.206 Materials for Artificial Blood Vessel Fabrication The basic element to construct a vascular graft is bulk material. Natural polymers (e.g., collagen, cellulose, chitosan, gelatin, silk, decellularized extracellular matrix) have good biocompatibility, bioactive functions, and friendly degradation. They are an ideal scaffold for tissue-engineered/bioactive grafts, but the compositions vary with batches and the mechanical strength is weak. Synthetic materials provide a variety of alternatives and include non-resorbable materials (e.g., polytetrafluoroethylene (PTFE), polyethylene terephthalate (PET), poly(ethylene glycol) (PEG)), resorbable materials (e.g., poly(ε-caprolactone) (PCL), poly(glycerol sebacate) (PGS), polyurethane (PU), thermoplastic polyurethane (TPU), poly(d, l-lactic acid-co-glycolic acid) (PLGA), polyglycolic acid (PGA), polylactic acid (PLA), poly(l-lactic acid) (PLLA), gelatin methacrylate-GelMA). [70,72,73]. Along with both types of polymers, different fabrication methods have been developed, as is shown in Figure 1.5, including braiding and knitting, paste extrusion and expansion, electrospinning, gas foaming/ particle leaching, 3D printing, cell-sheet engineering, and decellularization [74,75].
Biomaterials and Materials for Medicine
FIGURE 1.5 Commonly used methods for artificial blood vessel fabrication. (a) Braiding, (b) electrospinning, (c) extrusion, (d) gas foaming/particle leaching, (e) 3D printing, (f) Cellsheet engineering, and (g) decellularization.
Normally, two or more mentioned approaches are adopted. However, the biocompatibility of synthetic material is limited and some exhibit mechanical issues such as incompatible compliance. Increasing fiber diameter and the porosity of the PCL sheath increase the mechanical properties and promote graft vascular remodeling . United with rapid resorbable PGS core, the intima layer encourages vascular cell infiltration and matrix deposition to realize rapid cellularization . For a woven graft such as PGA, looser braids lead to bleeding and early rupture due to no structural support during degradation. Moreover, changing braiding density and angle result in a different level of inflammation, elastin/collagen deposition, and neovessel distensibility . Non-woven graft (ePTFE) is a node-fibril structure, and increasing the porosity from less than 30 μm to larger than 45 μm greatly facilitates cell engagement and growth without blood leakage . In the setting of hemodialysis patients, an elastic layer inserted between two ePTFE layers prevents puncturecaused bleeding and allows early cannulation within 24 hours . Furthermore, a sinusoidal architecture has been found to reach a mechanical strength close to the native blood vessel . Therefore, both the mechanical strength and the limited biocompatibility of synthetic materials, especially anticoagulation and neo-tissue formation, can be adjusted to a certain extent through modulating the polymers’ structure and composition . So far, the most commonly used clinical vascular graft materials are Dacron (PET), ePTFE, polyurethane (PU), and natural silk. 220.127.116.11 Surface Modification Technologies Surface property is another key element for a vascular graft as the substrate surface directly interacts with blood flow and native tissue to regulate the cellular events. The surface biocompatibility can be adjusted by physicochemical and
Cardiovascular Therapeutic Devices
bioactive modifications: (1) hydrophilic and hydrophobic surfaces , both of which can prevent the interaction between graft surface and blood components to reduce coagulation risk as the hydrophilic surface has a low interfacial free energy with blood and the hydrophobic surface has low surface energy ; (2) negative charge surface : electrostatic repulsion method is based negative cell surfaces and some negative proteins such as negative ePTFE and PET surfaces; however, the immediate uncontrolled protein absorption may disturb this anti-foul process. Additionally, both (1) and (2) methods may inhibit the protein-mediated cell adhesion and proliferation; (3) microphase separation surface : this kind of structure camouflages itself into a native material by inducing a site-selective absorption to different proteins; (4) grafting bioactive materials like heparin for anticoagulation, urokinase for fibrinolysis, or grafting bioactive group containing materials like sulfonic and carboxyl group ; (5) endothelialization: endothelial cells are a natural blood vessel barrier with ideal biofunction, a layer of which enhances biocompatibility, especially hemocompatibility. This layer can be realized either by seeding cells in vitro  or by presenting homing surfaces (e.g., RGD, VEGF) to recruit cells in vivo [74,86]. The latter one tends to provide a long-term functional cell layer. 18.104.22.168 Possibilities of Small Diameter Artificial Blood Vessel Artificial blood vessels of diameter equal to and larger than 6 mm have been successfully commercialized for clinical use (e.g., Atrium Advanta and Flixene (Atrium Medical Co.), Vascuted-Terumo (Vascutek), Impra & Venaflo & Carbodlo & Vectra (Bard Peripheral Vascular INC), Propaten & Gore-Tex (W.L.Gore & Associates), HeRO (Merit Medical), Acuseal (W.L. Gore)) . However, the development of small diameter artificial graft (less than 6 mm such as coronary artery bypass graft) remains a worldwide challenge. The compliance of widely used materials such as ePTFE, PET, PU, and PCL is not compatible with small vessels, which is always accompanied by calcification and inflammation-induced unexpected degradation. Moreover, the mismatched mechanical property together with low blood flow raises the risk of occlusive thrombus and can lead to hyperplasia [88–90]. In addition to the above-mentioned issues, there has been almost no change in the commonly used synthetic materials in the past 60 years, and the new generation of vascular graft materials have developed slowly. Therefore, manufacturing small vascular graft demands bulk material, fabrication, and surface modification. Currently, a hybrid or tissue-engineered small diameter graft has gained a significant advantage on patency. Through biomimicking the role of SMCs in maintaining vessel homeostasis, Wang et al. bio-fabricated an elastic vessel wall in PGA scaffold using SMCs differentiated from adipose-derived stem cells . Based on the native vessel wall structure, Chenxi et al. constructed a three-layered graft of 2–4 mm using silk and PU: a thin dense PU intima, a thick elastic textile-PU media, and a porous silk-PU adventitia, which showed a high patency rate and is ready for clinical trial . Wang et al. designed a nanotopographic intima surface to inhibit platelet adherence and activation . Moreover, to ensure a native intima-like layer, Yamanaka et al. decellularized a rat rail artery of 0.6 mm and modified the surface with synthesized peptide for rapid reendothelialization . Xu et al. constructed a
Biomaterials and Materials for Medicine
4 mm bilayer graft of both endothelial and SMCs via 3D printing . The National Cerebral and Cardiovascular Center of Japan has worked out a special approach to in situ construction. This group deployed a 0.6 mm stainless steel wire to successfully fabricate 0.6 mm collagen tubes in vivo. After transplantation, no thrombus was observed for 6 months. Recently, Yamamoto et al. revealed that shear stress (15 dynes/cm2) activated mitochondrial ATP production of endothelial cells, and thereby the production of vasodilator and nitric oxide via Ca2+ signaling . In this context, other key anticoagulation mechanism(s) may exist for small diameter native vessel if low shear stress failed to decrease cell membrane cholesterol. These results show great potential for brain and heart bypasses. Now, the thinnest vascular graft is around 3 mm. Only Atrium Medical Co. and Bard produce commercialized small vascular grafts. Theoretically, tissue-engineered graft is a promising approach for small diameter graft ; however, the production still requires further improvement in design and manufacturing techniques.
1.4 DEVICES FOR RESTORING CARDIAC HEMODYNAMICS Valve conditions and HF seriously impede normal blood supply. For pathological valves (e.g., regurgitation and stenosis), valve substitutes, repair, or percutaneous techniques have been applied to resolve the conditions (Figure 1.6 (left)). Regarding valve replacement, numerous developers focus on the design and optimization of artificial valves (referring to the mechanical valve, biological, as well as tissueengineering ones) for optimal therapeutic performance, high durability, low risk of thrombotic complications, and ideal hemodynamics. For treating HF, the gold standard, cardiac transplantation, is governed by the source and preservation of donor’s heart (Figure 1.6 (right)). Based on this setting, total artificial heart and ventricular assist have attracted the attention of researchers. Generally, considering device
FIGURE 1.6 Typical treatments of valvular diseases (left) and heart failure (right). The heart picture in middle is from 3DBody6.0 (Free).
Cardiovascular Therapeutic Devices
design and appropriate materials, excellent properties can be obtained, including good durability, smaller size or weight, and biocompatibility for human tissue.
1.4.1 Artificial Heart Valves Replacement Heart valves, including pulmonary valve, tricuspid valve, aortic valve, and mitral valve, can control the flow of blood through the chamber and prevent blood reflux through the valve’s “opening-closing” function. Heart valve conditions, routinely dedicated by coronary artery disease, high blood pressure, previous heart attack, or cardiomyopathy, can be resolved with valve replacement (pathological valve including regurgitation and stenosis are displaced by artificial valves), valve repair (normalizing a regurgitant valve surgically but not replacing), as well as percutaneous techniques covering percutaneous balloon valvuloplasty and transcatheter aortic valve implantation. This section discusses valves for cardiac valve replacement, primarily including mechanical valves and biological ones, the two most widely used implant valves to date. The former has the risk of thrombosis, while the latter is mainly about durability. More recent tissue-engineered valves are also discussed. 22.214.171.124 Mechanical Valves Mechanical valves, which appeared in the 1950s, made of artificial material and comprising sewing ring, occlusion, and retaining mechanism, possessed long-term durability but high clotting risk. For common candidates, ball-cage (the earliest artificial valves), tilting disk, and bileaflet (such as the Sorin Bicarbon valve) valves were designed. Artificial materials for mechanical valves originate from metal, ceramic, and polymer (e.g., stainless steel alloys, molybdenum alloys, titanium, silicone, and pyrolytic carbon) . As a typical foreign object, mechanical valves encounter thrombus, hemolysis, even resultant severe embolism and mechanical obstruction, which are induced by abnormal blood flow (including high shear stress, stagnant flow, and turbulence) related to valves’ implantation and their foreign surface. Therefore, using anticoagulants (such as warfarin potassium) or lowering clotting surface or new valve design is obligatory. Patients receiving blood thinners suffer from high bleeding risk. With weakening adverse effects, coating techniques have paved the way for the ameliorative hemocompatibility of devices. As summarized by Wheatley et al., surface treatments, carbon-based coatings (e.g., depositing diamondlike carbon (DLC) coating), fluoridization, plasma and glow discharge treatment, or oxidation post-treatments, generated thrombus eradicated surface marked by fewer platelets and reduced thrombosis [99,100]. In one example, Major et al. deposited a C:H-based coating onto the thermoplastic polyurethane (TPU) substrates and subsequently confirmed that the coating could be used in blood contact circumstances with a high value of shear stress potently, increased hemocompatibility, and without causing an immune response . More than surface modification, meeting mechanical design (mechanical safety) of valves and physiological requirements of the organism, new valve designs also have been attainable. Flexible valves, partly simulating native valves, guide similar hemodynamics to biological valves. Textile valves with available flexible leaflets acquire blood flow similar to natural valves with adjustable durability . Different materials and manufacturing methods
Biomaterials and Materials for Medicine
have been vigorously investigated, such as PET textile materials and polyester textiles [102,103]. Polynova valves provide high durability as well as low thrombogenicity, as reported by Piatti et al. . 126.96.36.199 Tissue Valves Considering that the heart valves withstand repetitive “opening/closing” action about 31,536,000 times per year, high durability needs to be considered . Tissue heart valves require a donor (actual valves or tissue), such as porcine (pig), bovine (cow), horse, or human, and last 10–15 years ordinarily after placing in the body , categorized as xenografts, allografts, and homografts. Compared with mechanical valves, bioprosthetic valves naturally instigate a more physiological blood flow with reduced clotting after replacing, while not succeeding durability and failing to meet mechanical requirements compromised by structural degradation connecting to immunoreaction and calcification . Several studies have established that degeneration of tissue valves is caused by recipient and donor factors (age, disease, allograft size, body surface area of receiver), sterilization and preservation methods, and implantation techniques [107–109]. In adults, it is widely accepted that the durability of an allograft is equal to or better than that of manual bioprostheses, and slow fibrocalcific degeneration stimulates its failure . Simultaneously, of note, allograft valves have ideal performance followed by normal hemodynamics and excellent freedom from infectious endocarditis and thromboembolism . For allografts, the specificity of transplanted tissue can elicit an immune response, which touches on the service life of bio-valves. Compared with standard cryopreserved valved allografts, decellularized cryopreserved valve allografts with lower immunogenicity and higher durability displayed better mid-term performance in an approximately 5-year study . Theoretically, thorough detachment of cellular components (cell and cellular debris) from donor tissue can lower the immunogenicity of implants, which makes implants reconfigure. Further, the remodeled patient-adapted valves can enhance durability and ameliorate degeneration and calcification . Helder et al. also mentioned that acellular allografting, exhibiting fibrosis and calcification in explanted produce failure models such as standard valves, which are driven by tissue damaging through decellularization process and sterilization procedure . A cryopreserved homograft is a valid option  because they are an imperfect but satisfactory biological material for reconstructing natural outflow . Moreover, for more optimal biofunctional answering after explanting, decorating decellularized homografts have been built. In clinical practices, the problems of calcification and intimal hyperplasia impeded the outcomes of cryopreserved homografts, coating of fibronectin and stromal cell-derived factor-1a onto the cell-free ovine aortic homografts inhibited immune reaction mediated by cryopreserved heart valve, calcification, pannus formation, and accelerated re-endothelialization . 188.8.131.52 Tissue-Engineered Valves Some significant advancements have been witnessed in valve explanting, from first mechanical valves and bioprosthetic valves to tissue-engineered valves. On the premise of more physiological flow patterns and affirmative blood compatibility, tissue-engineered heart valves (TEHVs) harvest durability of mechanical valves, the
Cardiovascular Therapeutic Devices
hemodynamic performance of biological valves, and regenerative ability of native tissues intelligently, eventually obtain the patients’ valves with biocompatibility. Multitudinous TEHVs have been devised for developing “living” valves with favorable cell ingrowth and tissue remodeling, such as a scaffold integrating autologous bone marrow-derived mononuclear cells and biodegradable matrix . Currently, various materials have been applied for scaffold fabrication, including natural materials (fibrin and collagen), polymeric substance (e.g., PGA and PLA or their co-polymers, and PEG-DA) and ECM from decellularized engineered tissue and decellularized donor valves [119–122]. More than materials, newer valve design emerged. In one example, Reimer and colleagues developed a tubular heart valve stemming from two cell-free extracellular matrix tubes with organized collagenous matrix. After that, exceeding recellularization and, ideally, somatic growth, these valves exhibited full leaflet opening and closing, minimal regurgitation under simulated physiological conditions, and no tissue damage after 2 million cycles of fatigue testing . Cell-seeded TEHVs are another alternative. Coupling fibrin-based valves supporter and cells originating from ovine carotid artery demonstrated improved seeded cell adhesion and alignment in fibrin substrate, tuned ECM producing, and remodeled the valve matrix under given dynamic conditioning . For cell-based biodegradable scaffolds, mechanical properties are dramatically determined by lost mechanical properties due to biodegradation of the scaffolds and additional counterparts involving de-novo matrix synthesis. According to Sant et al., valvular interstitial cells (VICs) entrapped into PGS–PCL (fast degrading polyglycerol sebacate (PGS) and slowly degrading polycaprolactone (PCL)) scaffolds secreted new matrix protein for rebuilding the synthetic scaffold during the old one degrading, which kept the scaffolds stable . Over these, in light of structural and anisotropic mechanical characteristics of the native valve leaflets, manufacturing technologies for TEHVs are also a major research field. Existing options include bioengineering methods (decellularizing and conditioning valves successively), which reduced antigenicity and generated comparative hemodynamical with intrinsic valves ; multiple-step injection molding, which provided high integrity ; electrospinning and microfabrication techniques, which can also mimic mechanism and unique mechanical features . Altogether, excimer laser microfabrication and predictive modeling are also candidates . Decellularized heart valves (xenogenic or allogenic)  and remolded collagenous organization  by primitive fibrin gel holder replaced primitive cell-produced collagenous matrix served as starter matrix.
1.4.2 Heart Function Recovery HF has high mortality as the 10-year lethal rates are 89% and 86% in men and women aged 65–74 years, respectively . Cardiac transplantation, the gold standard for treating end-stage HF, is a highly effective solution to settle end‐stage HF, but limited by the unavailability of heart donors. This drawback initiates the growing use of mechanical circulatory support. This part extensively focused on the total artificial heart and ventricular assist device (VAD) implantation, the two main options to remedy end‐stage HF. Implanting a VAD also potently renews heart function, even though the device is not considered to last the entire lifecycle . A large number
Biomaterials and Materials for Medicine
of studies have proven that, in addition to the material itself, the hemodynamic characteristics after implantation of artificial ventricle affect the service performance of the device. Usually, hemodynamics evoke blood damage embracing different mechanisms, such as hemolysis, platelet activation, thrombosis, and emboli . Given these, more than selected materials for artificial heart and VAD, extended substantial advancements have achieved optimized mechanical design. 184.108.40.206 Totally Artificial Heart Heart transplantation is regarded as the most effective treatment for patients suffering from end-stage HF; however, unfortunately, it is obstructed by organ shortage and the source of donors. These drawbacks drive the booming of the artificial heart to minimize the need for donor hearts. Currently, total artificial heart (TAH) systems involve three blocks: pump units featuring limited durability, percutaneous tubes, as well as bulky external equipment . The TAH is an extremely important curative option withstanding serious biventricular dysfunction or other aggravated structural abnormalities. From the pioneering era to date, several TAH systems have emerged. CardioWest TAH (SynCardia Systems, Inc., Tucson, AZ), the only commercially available TAH in the United States approved by the FDA, was marked completely in 2004 . Copeland et al. stated that the CardioWest TAH can reduce these problems (e.g., right HF, valvular regurgitation, cardiac arrhythmias, ventricular clots) after implanting left ventricular and biventricular assist devices . The AbioCor TAH, another FDA-approved TAH in 2006 , totally implantable, was similar to the Syncardia device with similar graft and cuff design , and was motor-driven without percutaneous cables, conduits, or wires . The Carmat total artificial heart (C-TAH, Vélizy-Villacoublay, France), a newer heart replacement device described as an electro-hydraulically driven, pulsatile biventricular pump support containing bioprosthetic blood-contacting surfaces, was designed to weaken thromboembolism events and bleeding and save lives. The first clinical use of a bioprosthetic C-TAH has been accepted after extensive investigation. C-TAH contains ventricles, each with a blood compartment and a hydraulic fluid working on drive unit parted by hybrid membranes coming from ePTFE and bovine pericardial tissue [138,139]. Naturally, hemocompatibility and safety of hybrid membranes are vital for the performance of this device. The safety of hybrid membrane confirmed insignificant change in mechanical, physical, and chemical properties from 9 months up to 4 years of aging, eliminate membrane calcification, and no hemolysis trigger and platelet sensitization . Markedly, over physiological blood dynamics, after using C-TAH, the progressive endothelialization of C-TAH has been demonstrated . Pivotally, the C-TAH equipped with autoregulated mode encouraged endothelial homeostasis preservation . The ReinHeart TAH, an electrically driven and fully implantable Destination Therapy TAH system, owns strong preload sensitivity and guides the integration of physiologic flow control [132,143]. 220.127.116.11 Ventricular Assist Devices (VADs) Today, over 2,000 patients receive mechanical circulatory devices annually in the United States, which relieve the pressure on the donor source . VADs, a prospective lifesaving equipment, consisting of electrically powered pumps (circulating
Cardiovascular Therapeutic Devices
blood), controller unit (monitoring, and controlling the previous part), and power unit (supply electricity for the device), are applied to support patients until heart donation (termed as bridge‐to transplantation (BTT)) or recover essential cardiac function during/after heart surgery (named as bridge‐to‐recovery (BTR)) [145,146]. Additionally, for destination therapy (DT), VADs also have been utilized to substitute for cardiac transplantation, permanent, or long-term application to the human body . It has been seen that the usage of VADs promotes the survival rate of suffers. The study conducted by Burns and team revealed that implanting of a left ventricular assist device (LVAD) germinate beneficial reverse remodeling of myocardial structure and function . VADs are divided into three categories, named LVAD, right ventricular assist device, as well as biventricular assist device . The evolution of implantable blood pumps follows the rules of smaller size, lower thrombosis rate and hemolysis, high durability, fewer accessories, and low risk of postoperative infection. Progressively, first‐generation VADs with pulsatile pump had limitations such as short of huge volume and blood-contacting surfaces, pro-thrombosis effects, poor durability, and infection. For thrombosis, anticoagulant therapy is necessary such as aspirin for lifelong administration after VAD implantation . Further second-generation products with smaller size and high durability, engendered continuous, unidirectional blood flow, induced by their centrifugal, axial, or hybrid pumps. Seeing that hemolysis caused by contact bearings, more recent third‐generation VADs use “non-contact”-bearing design, which resulted in a durable device, rapid postoperative recovery, less hemolysis, and thrombosis [130,145,150,151]. At present, implantable VAD suitable for multifarious attempts are obtainable commercially, as Heart Assist 5, Heart Mate II, and Jarvik-2000 belonging to second-generation pumps and Dura Heart belonging to third generation pump . Technically, wireless transfer technology with more reliable and longer transmission distance has greatly promoted the development of mechanical circulatory supporters .
REFERENCES 1. G.E. Cimochowski, R.H. Evans, C.K. Zarins, C.T. Lu, T.R. DeMeester. Greenfield filter versus Mobin-Uddin umbrella: The continuing quest for the ideal method of vena cava interruption. J. Thorac. Cardiovasc. Surg. 79 (1980) 358–365. doi:10.1016/ s0022-5223(19)37944-9. 2. Q. Chau, S.B. Cantor, E. Caramel, M. Hicks, D. Kurtin, T. Grover, L.S. Elting. Costeffectiveness of the bird’s nest filter for preventing pulmonary embolism among patients with malignant brain tumors and deep venous thrombosis of the lower extremities. Support. Care Cancer. 11 (2003) 795–799. doi:10.1007/s00520-003-0520-2. 3. H.J. Jaeger, S. Kolb, T. Mair, M. Geller, A. Christmann, R.K.H. Kinne, K.D. Mathias. In vitro model for the evaluation of inferior vena cava filters: Effect of experimental parameters on thrombus-capturing efficacy of the Vena Tech- LGM filter. J. Vasc. Interv. Radiol. 9 (1998) 295–304. doi:10.1016/S1051-0443(98)70272-6. 4. P.A. Poletti, C.D. Becker, L. Prina, P. Ruijs, H. Bounameaux, D. Didier, P.A. Schneider, F. Terrier. Long-term results of the Simon nitinol inferior vena cava filter. Eur. Radiol. 8 (1998) 289–294. doi:10.1007/s003300050382. 5. R.L. Leask, K.W. Johnston, M. Ojha. Hemodynamic effects of clot entrapment in the trapease inferior vena cava filter. J. Vasc. Interv. Radiol. 15 (2004) 485–490. doi:10.1097/01. RVI.0000124941.58200.85.
Biomaterials and Materials for Medicine
6. N.Y. Yim, N.K. Chang, J.H. Lim, J.K. Kim. Retrograde tempofilter IITM placement within the superior vena cava in a patient with acute upper extremity deep venous thrombosis: The filter stands on its head. Korean J. Radiol. 12 (2011) 140–143. doi:10.3348/ kjr.2011.12.1.140. 7. S. Wicky, F. Doenz, J.Y. Meuwly, F. Portier, P. Schnyder, A. Denys. Clinical experience with retrievable Günther Tulip vena cava filters. J. Endovasc. Ther. 10 (2003) 994–1000. doi:10.1583/1545-1550(2003)0102.0.CO;2. 8. S.W. Stavropoulos, J.X. Chen, R.F. Sing, F. Elmasri, M.J. Silver, A. Powell, F.C. Lynch, A.K. Abdel Aal, A. Lansky, B.E. Muhs. Analysis of the final DENALI trial data: A prospective, multicenter study of the Denali inferior vena cava filter. J. Vasc. Interv. Radiol. 27 (2016) 1531–1538.e1. doi:10.1016/j.jvir.2016.06.028. 9. J.C. Durack, A.C. Westphalen, S. Kekulawela, S.B. Bhanu, D.E. Avrin, R.L. Gordon, R.K. Kerlan. Perforation of the IVC: Rule rather than exception after longer indwelling times for the günther tulip and celect Retrievable Filters. Cardiovasc. Intervent. Radiol. 35 (2012) 299–308. doi:10.1007/s00270-011-0151-9. 10. H.B. Smouse, R. Mendes, M. Bosiers, T.G. Van Ha, T. Crabtree. The RETRIEVE trial: Safety and effectiveness of the retrievable crux vena cava filter. J. Vasc. Interv. Radiol. 24 (2013) 609–621. doi:10.1016/j.jvir.2013.01.489. 11. X. Zhang, B.H. Tan, Z. Li. Biodegradable polyester shape memory polymers: Recent advances in design, material properties and applications. Mater. Sci. Eng. C. 92 (2018) 1061–1074. doi:10.1016/j.msec.2017.11.008. 12. Q. Zhao, H.J. Qi, T. Xie. Recent progress in shape memory polymer: New behavior, enabling materials, and mechanistic understanding. Prog. Polym. Sci. 49–50 (2015) 79–120. doi:10.1016/j.progpolymsci.2015.04.001. 13. R.K. Avery, H. Albadawi, M. Akbari, Y.S. Zhang, M.J. Duggan, D. V. Sahani, B.D. Olsen, A. Khademhosseini, R. Oklu. An injectable shear-thinning biomaterial for endovascular embolization. Sci. Transl. Med. 8 (2016) 365ra156. doi:10.1126/scitranslmed.aah5533. 14. H. Jiang, J.P. Wang, Y.C. Li, Y.Y. Tong, Q. Yang, D. Yan, L.L. Ding, S.G. Yuan. Experimental study of vascular embolization with homemade second-level Copper coil. Chinese J. Radiol. 47 (2013) 183–187. doi:10.3760/cma.j.issn.1005-1201.2013.02.018. 15. H. Zhengsong, D. Qinshun, J. Tao, L. Junshi. Endovascular embolization of intracranial aneurysms with self-made tungsten coils in a dog model. Chin. Med. J. (Engl). 109 (1996) 626–630. doi:10.3171/jns.2004.101.6.0996. 16. A. Kurata, S. Suzuki, H. Ozawa, I. Yuzawa, M. Yamda, K. Fujii, S. Kan, T. Kitahara, T. Ohmomo, Y. Miyasaka. Application of the liquid coil as an embolic material for arteriovenous malformations. Interv. Neuroradiol. 11 (2005) 287–295. doi:10.1177/ 159101990501100315. 17. C.B. Luo, M.M.H. Teng, F.C. Chang, C.Y. Chang. Endovascular treatment of intracranial high-flow arteriovenous fistulas by Guglielmi detachable coils. J. Chinese Med. Assoc. 69 (2006) 80–85. doi:10.1016/S1726-4901(09)70118-2. 18. S. Albayram, D. Selcuk, A. Soeda, N. Sakai, K. Iihara, I. Nagata. Thromboembolic events associated with Guglielmi detachable coil embolization of asymptomatic cerebral aneurysms: Evaluation of 66 consecutive cases with use of diffusion-weighted MR imaging  (multiple letters). Am. J. Neuroradiol. 25 (2004) 159–160. PMID: 12533341. 19. W. Möller-Hartmann, T. Krings, K. Stein, H. Dreeskamp, A. Meetz, F.J. Hans, R. Thiex, J. Gilsbach, A. Thron. Treatment of experimental aneurysms in rabbits using Guglielmi detachable coils: A feasibility study. Riv. Di Neuroradiol. 16 (2003) 1154–1156. doi:10.1177/ 197140090301600631. 20. A. Tournade, P. Courtheoux, C. Sengel, S. Ozgulle, T. Tajahmady. Saccular intracranial aneurysms: Endovascular treatment with mechanical detachable spiral coils. Radiology. 202 (1997) 481–486. doi:10.1148/radiology.202.2.9015078.
Cardiovascular Therapeutic Devices
21. H. Kiyosue, H. Mori, S. Matsumoto, Y. Hori, M. Okahara, S. Tanoue, Y. Sagara. Clinical use of a new mechanical detachable coil system for percutaneous intravenous embolization of cavernous sinus dural arteriovenous fistulas. Radiat. Med. - Med. Imaging Radiat. Oncol. 22 (2004) 143–147. PMID: 15287528. 22. A. Kinoshita, M. Ito, T. Skakaguchi, K. Yamada, S. Akizuki, M. Taneda, T. Hayakawa. Mechanical detachable coil as a therapeutic alternative for cerebral aneurysm. Neurol. Res. 16 (1994) 475–476. doi:10.1080/01616412.1994.11740277. 23. H.J. Cloft, D.F. Kallmes. Aneurysm packing with hydrocoil embolic system versus platinum coils: Initial clinical experience. Am. J. Neuroradiol. 25 (2004) 60–62. PMID: 14729529. 24. B.R. Bendok, K.R. Abi-Aad, J.D. Ward, J.F. Kniss, M.J. Kwasny, R.J. Rahme, S.G. Aoun, T.Y. El Ahmadieh, N.E. El Tecle, S.G. Zammar, R.J.N. Aoun, D.P. Patra, S.A. Ansari, J. Raymond, H.H. Woo, D. Fiorella, G. Dabus, G. Milot, J.E. Delgado Almandoz, J.A. Scott, A.J. Denardo, S.R. Dashti, S. Ansari, E. Deshaies, S. Lavine, H. Bozorgchami, J. Delgado, E. Veznedaroglu, F. Albuquerque, D. Fiorella, A. Boulos, M. Cortes, H. Kanaan, G. Jindal, R. Klucznik, G. Dabus, D. Kalmes, R. Tawk, J. Raymond, C. Romero, A. Xavier, M. Hussain, M. Kelly, C. Moran, I. Chaudry, A. Pandey, D. Wang, B. Van Adel, G. Milot, J. Hirsch, J. Carpenter, C. Powers, P. Jabbour, G. Luh, J. Shankar, R. Tummala, A. Patsalides, A. Evans, A. Garg, S. Dashti, S. Lee, R. James, M. Jayaraman, S. Satti, E. Sauvageau, J. Fields, T. Grobelny, J. Hartman. The Hydrogel Endovascular Aneurysm Treatment Trial (HEAT): A randomized controlled trial of the second-generation hydrogel coil. Neurosurgery. 86 (2020) 615–624. doi:10.1093/neuros/nyaa006. 25. W. Zhi-Gang, D. Xuan, Z. Ji-Qing, Q. Chun-Cheng, W. Cheng-Wei, H. De-Zhang, H. Xiao-Guang. HydroCoil occlusion for treatment of traumatic carotid-cavernous fistula: Preliminary experience. Eur. J. Radiol. 71 (2009) 456–460. doi:10.1016/j. ejrad.2008.06.009. 26. Y. Murayama, F. Viñuela, A. Ishii, Y.L. Nien, I. Yuki, G. Duckwiler, R. Jahan, Initial clinical experience with Matrix detachable coils for the treatment of intracranial aneurysms, J. Neurosurg. 105 (2006) 192–199. 27. L. Zhou, B. Zhong, H. Du, W. Wang, J. Shen, S. Zhang, W. Li, H. Tang, P. Zhang, W. Yang, X. Zhu. Comparison of embolic agents for varices during transjugular intrahepatic portosystemic shunt for variceal bleeding: Tissue gel or coil? J. Interv. Med. 3 (2020) 195–200. doi:10.1016/j.jimed.2020.08.008. 28. W. Brinjikji, A.P. Amar, J.E. Delgado Almandoz, O. Diaz, P. Jabbour, R. Hanel, F. Hui, M. Kelly, K.D. Layton, J.W. Miller, E. Levy, C. Moran, D.C. Suh, H. Woo, R. Sellar, B. Hoh, A. Evans, D.F. Kallmes. GEL THE NEC: A prospective registry evaluating the safety, ease of use, and efficacy of the HydroSoft coil as a finishing device. J. Neurointerv. Surg. 10 (2018) 83–87. doi:10.1136/neurintsurg-2016-012915. 29. N. Wang, X. Jiang, J. Wang, X. Hao, Study on the application of embolization materials of collagen, in: IOP Conf. Ser. Mater. Sci. Eng., 2019: pp. 012005. doi:10.1088/1757-899X/ 587/1/012005. 30. J.J. Rong, D. Liu, M. Liang, Q.H. Wang, J.Y. Sun, Q.Y. Zhang, C.F. Peng, F.Q. Xuan, L.J. Zhao, X.X. Tian, Y.L. Han. The impacts of different embolization techniques on splenic artery embolization for blunt splenic injury: A systematic review and metaanalysis. Mil. Med. Res. 4 (2017). doi:10.1186/s40779-017-0125-6. 31. A.R. Grüntzig, Å. Senning, W.E. Siegenthaler. Nonoperative dilatation of coronaryartery stenosis - percutaneous transluminal coronary angioplasty. N. Engl. J. Med. 301 (1979) 61–68. doi:10.1056/nejm197907123010201. 32. R. Lowe, I.B.A. Menown, G. Nogareda, I.M. Penn. Coronary stents: In these days of climate change should all stents wear coats?. Heart. 91 (2005) 20–23. doi:10.1136/ hrt.2005.060269.
Biomaterials and Materials for Medicine
33. I. Cockerill, C.W. See, M.L. Young, Y. Wang, D. Zhu. Designing better cardiovascular stent materials: A learning curve. Adv. Funct. Mater. 2005361 (2020) 1–23. doi:10.1002/ adfm.202005361. 34. R. Wessely. New drug-eluting stent concepts. Nat. Rev. Cardiol. 7 (2010) 194–203. doi:10.1038/nrcardio.2010.14. 35. K. Dan, E. Shlofmitz, N. Khalid, A. Hideo-Kajita, J.P. Wermers, R. Torguson, P. Kolm, H.M. Garcia-Garcia, R. Waksman. Paclitaxel-related balloons and stents for the treatment of peripheral artery disease: Insights from the Food and Drug Administration 2019 Circulatory System Devices Panel Meeting on late mortality: Paclitaxel devices in PAD treatment. Am. Heart J. 222 (2020) 112–120. doi:10.1016/j.ahj.2019.12.012. 36. J. Pache, A. Kastrati, J. Mehilli, H. Schühlen, F. Dotzer, J. Hausleiter, M. Fleckenstein, F.J. Neuman, U. Sattelberger, C. Schmitt, M. Müller, J. Dirschinger, A. Schömig. Intracoronary stenting and angiographic results: Strut thickness effect on restenosis outcome (ISAR-STEREO-2) trial. J. Am. Coll. Cardiol. 41 (2003) 1283–1288. doi:10.1016/S0735-1097(03)00119-0. 37. A. Lansky, W. Wijns, B. Xu, H. Kelbæk, N. van Royen, M. Zheng, M. Morel, P. Knaapen, T. Slagboom, T.W. Johnson, G. Vlachojannis, K.E. Arkenbout, L. Holmvang, L. Janssens, A. Ochala, S. Brugaletta, C.K. Naber, R. Anderson, H. Rittger, S. Berti, E. Barbato, G.G. Toth, L. Maillard, C. Valina, P. Buszman, H. Thiele, V. Schächinger, A. Baumbach. Targeted therapy with a localised abluminal groove, low-dose sirolimus-eluting, biodegradable polymer coronary stent (TARGET All Comers): A multicentre, open-label, randomised non-inferiority trial. Lancet. 392 (2018) 1117–1126. doi:10.1016/S0140-6736(18)31649-0. 38. Y.J. Zhang, F. Chen, T. Muramatsu, B. Xu, Z.Q. Li, J.B. Ge, Q. He, Z.J. Yang, S.M. Li, L.F. Wang, H.C. Wang, B. He, K. Li, G.X. Qi, T.C. Li, H.S. Zeng, J.J. Peng, T.M. Jiang, Q.T. Zeng, J.H. Zhu, G.S. Fu, C. V. Bourantas, P.W. Serruys, Y. Huo. Nine-month angio graphic and two-year clinical follow-up of polymer-free sirolimus-eluting stent versus durable-polymer sirolimus-eluting stent for coronary artery disease: The nano randomized trial. Chin. Med. J. (Engl). 127 (2014) 2153–2158. doi:10.3760/ cma.j.issn.0366-6999.20133148. 39. Y. Katagiri, P.W. Serruys, T. Asano, Y. Miyazaki, P. Chichareon, R. Modolo, K. Takahashi, N. Kogame, J.J. Wykrzykowska, J.J. Piek, Y. Onuma, A. Kastrati. How does the failure of absorb apply to the other bioresorbable scaffolds? An expert review of first-in-man and pivotal trials. EuroIntervention. 15 (2019) 116–123. doi:10.4244/EIJ-D-18-00607. 40. C. Beyan, E. Beyan. Bioresorbable scaffolds: Current technology and future perspectives. Rambam Maimonides Med. J. 11 (2020) e0039. doi:10.5041/RMMJ.10402. 41. E. Mostaed, M. Sikora-Jasinska, J.W. Drelich, M. Vedani. Zinc-based alloys for degradable vascular stent applications. Acta Biomater. 71 (2018) 1–23. doi:10.1016/j. actbio.2018.03.005. 42. R.M. Waksman, PROGRESS was made toward DREAM: Magnesium Stent, report in Washington hospital center, 2012. https://bioflow.hu/dynamic/PROGRESS-to-DREAMSWaksman-20120517-1455-RoomMaillot.pdf. 43. M. Haude, H. Ince, A. Abizaid, R. Toelg, P.A. Lemos, C. Von Birgelen, E.H. Christiansen, W. Wijns, F.J. Neumann, C. Kaiser, E. Eeckhout, S.T. Lim, J. Escaned, H.M. Garcia-Garcia, R. Waksman. Safety and performance of the second-generation drug-eluting absorbable metal scaffold in patients with de-novo coronary artery lesions (BIOSOLVE-II): 6 month results of a prospective, multicenter, non-randomised, first-in-man trial. Lancet. 387 (2016) 31–39. doi:10.1016/S0140-6736(15)00447-X. 44. M. Haude, H. Ince, S. Kische, R. Toelg, N.M. Van Mieghem, S. Verheye, C. von Birgelen, E.H. Christiansen, E. Barbato, H.M. Garcia-Garcia, R. Waksman. Sustained safety and performance of the second-generation sirolimus-eluting absorbable metal scaffold: Pooled outcomes of the BIOSOLVE-II and -III trials at 3 years. Cardiovasc. Revascularization Med. 21 (2020) 1150–1154. doi:10.1016/j.carrev.2020.04.006.
Cardiovascular Therapeutic Devices
45. A.M. Galløe, H. Kelbæk, L. Thuesen, H.S. Hansen, J. Ravkilde, P.R. Hansen, E.H. Christiansen, U. Abildgaard, G. Stephansen, J.F. Lassen, T. Engstrøm, J.S. Jensen, J.L. Jeppesen, N. Bligaard, P. Thayssen, J. Aarøe, K. Saunamäki, A. Junker, H.H. Tilsted, H.E. Bøtker, S. Galatius, C.T. Larsen, S.D. Kristensen, L.R. Krusell, S.Z. Abildstrøm, M. Meng, L. Okkels. 10-Year clinical outcome after randomization to treatment by sirolimus- or paclitaxel-eluting coronary stents. J. Am. Coll. Cardiol. 69 (2017) 616– 624. doi:10.1016/j.jacc.2016.11.055. 46. N. Rajendra, B. Wrigley, A. Gershlick. Bioabsorbable stents: Nothing from something. Clin. Investig. (Lond). 2 (2012) 1185–1189. doi:10.4155/cli.12.126. 47. B. Scheller, U. Speck, C. Abramjuk, U. Bernhardt, M. Böhm, G. Nickenig. Paclitaxel balloon coating, a novel method for prevention and therapy of restenosis. Circulation. 110 (2004) 810–814. doi:10.1161/01.CIR.0000138929.71660.E0. 48. J.A. Anderson, S. Lamichhane, T. Remund, P. Kelly, G. Mani. Preparation, characterization, in vitro drug release, and cellular interactions of tailored paclitaxel releasing polyethylene oxide films for drug-coated balloons. Acta Biomater. 29 (2016) 333–351. doi:10.1016/j.actbio.2015.09.036. 49. A. De Labriolle, R. Pakala, L. Bonello, G. Lemesle. Interventional rounds paclitaxeleluting balloon : From bench to bed. Catheter. Cardiovasc. Interv. 652 (2009) 643–652. doi:10.1002/ccd.21895. 50. K.J. Lee, S.G. Lee, I. Jang, S.H. Park, D. Yang, I.H. Seo, S.K. Bong, D.H. An, M.K. Lee, I.K. Jung, Y.H. Jang, J.S. Kim, W.H. Ryu. Linear Micro-patterned Drug Eluting Balloon (LMDEB) for enhanced endovascular drug delivery. Sci. Rep. 8 (2018) 1–13. doi:10.1038/ s41598-018-21649-7. 51. C.D. Owens, W.J. Gasper, J.P. Walker, H.F. Alley, M.S. Conte, S.M. Grenon. Safety and feasibility of adjunctive dexamethasone infusion into the adventitia of the femoropopliteal artery following endovascular revascularization. J. Vasc. Surg. 59 (2014) 1016–1024. doi:10.1016/j.jvs.2013.10.051. 52. K.J. Lee, J.Y. Lee, S.G. Lee, S.H. Park, D.S. Yang, J.J. Lee, A. Khademhosseini, J.S. Kim, W.H. Ryu. Microneedle drug eluting balloon for enhanced drug delivery to vascular tissue. J. Control. Release. 321 (2020) 174–183. doi:10.1016/j.jconrel.2020.02.012. 53. J.A. Anderson, S. Lamichhane, K. Fuglsby, T. Remund, K. Pohlson, R. Evans, D. Engebretson, P. Kelly, S. Falls. Development of drug-coated balloon for the treatment of multiple peripheral artery segments. J. Vasc. Surg. 71 (2019) 1750–1757.e7. doi:10.1016/j.jvs.2019.04.494. 54. H. Ang, T.R. Koppara, S. Cassese, J. Ng, M. Joner, N. Foin. Drug-coated balloons: Technical and clinical progress. Vasc. Med. (United Kingdom). 25 (2020) 577–587. doi:10.1177/1358863X20927791. 55. C.A. Gongora, M. Shibuya, J.D. Wessler, J. McGregor, A. Tellez, Y. Cheng, G.B. Conditt, G.L. Kaluza, J.F. Granada. Impact of paclitaxel dose on tissue pharmacokinetics and vascular healing a comparative drug-coated balloon study in the familial hypercholesterolemic swine model of superficial femoral in-stent restenosis. JACC Cardiovasc. Interv. 8 (2015) 1115–1123. doi:10.1016/j.jcin.2015.03.020. 56. T. Heilmann, C. Richter, H. Noack, S. Post, D. Mahnkopf, A. Mittag, H. Thiele, F. HansReiner. Drug release profiles of different drug-coated balloon platforms. Eur. Cardiol. Rev. 6 (2010) 40. doi:10.15420/ecr.2010.8.2.40. 57. R. Iyer, A.E. Kuriakose, S. Yaman, L.C. Su, D. Shan, J. Yang, J. Liao, L. Tang, S. Banerjee, H. Xu, K.T. Nguyen. Nanoparticle eluting-angioplasty balloons to treat cardiovascular diseases. Elsevier B.V. 554 (2019) 212–223. doi:10.1016/j.ijpharm.2018.11.011. 58. T.R. Dugas, G. Brewer, M. Longwell, T. Fradella, J. Braun, C.E. Astete, M.H. Jennings, C.M. Sabliov. Nanoentrapped polyphenol coating for sustained drug release from a balloon catheter. J. Biomed. Mater. Res. - Part B Appl. Biomater. 107 (2019) 646–651. doi:10.1002/jbm.b.34157.
Biomaterials and Materials for Medicine
59. P.P. Buszman, A. Tellez, M.E. Afari, A. Peppas, G.B. Conditt, S.D. Rousselle, J.C. McGregor, M. Stenoien, G.L. Kaluza, J.F. Granada. Tissue uptake, distribution, and healing response after delivery of paclitaxel via second-generation iopromidebased balloon coating: A comparison with the first-generation technology in the iliofemoral porcine model. JACC Cardiovasc. Interv. 6 (2013) 883–890. doi:10.1016/j. jcin.2013.04.013. 60. G.H. Chang, D.A. Azar, C. Lyle, V.C. Chitalia, T. Shazly, V.B. Kolachalama. Intrinsic coating morphology modulates acute drug transfer in drug-coated balloon therapy. Sci. Rep. 9 (2019) 1–10. doi:10.1038/s41598-019-43095-9. 61. A.R. Tzafriri, S.A. Parikh, E.R. Edelman. Taking paclitaxel coated balloons to a higher level: Predicting coating dissolution kinetics, tissue retention and dosing dynamics. J. Control. Release. 310 (2019) 94–102. doi:10.1016/j.jconrel.2019.08.019. 62. U. Speck, B. Cremers, B. Kelsch, M. Biedermann, Y.P. Clever, S. Schaffner, D. Mahnkopf, U. Hanisch, M. Böhm, B. Scheller. Do pharmacokinetics explain persistent restenosis inhibition by a single dose of paclitaxel? Circ. Cardiovasc. Interv. 5 (2012) 392–400. doi:10.1161/CIRCINTERVENTIONS.111.967794. 63. P.M. Kitrou, K. Katsanos. Sirolimus-coated balloons for the treatment of femoropopliteal lesions: New player in the game? J. Endovasc. Ther. (2020). doi:10.1177/ 1526602820946377. 64. S. Basavarajaiah, S. Athukorala, K. Kalogeras, V. Panoulas, B.H. Loku Waduge, G. Bhatia, R. Watkin, G. Pulikal, K. Lee, J. Ment, B. Freestone, M. Pitt. Mid‐term clinical outcomes from use of sirolimus coated balloon in coronary intervention; data from real world population. Catheter. Cardiovasc. Interv. (2020) ccd.28998. doi:10.1002/ccd.28998. 65. H. Bin Liu, M. Byrne, P. Perlmutter, A. Walker, G.R. Sama, J. Subbiah, B. Ozcelik, R.E. Widdop, T.A. Gaspari, K. Byron, Y.C. Chen, D.M. Kaye, A.E. Dear. A novel epigenetic drug-eluting balloon angioplasty device: Evaluation in a large animal model of neointimal hyperplasia. Cardiovasc. Drugs Ther. 33 (2019) 687–692. doi:10.1007/ s10557-019-06921-w. 66. R. V. Jeger, S. Eccleshall, W.A. Wan Ahmad, J. Ge, T.C. Poerner, E.S. Shin, F. Alfonso, A. Latib, P.J. Ong, T.T. Rissanen, J. Saucedo, B. Scheller, F.X. Kleber. Drug-coated balloons for coronary artery disease: Third report of the international DCB consensus group. JACC Cardiovasc. Interv. 13 (2020) 1391–1402. doi:10.1016/j.jcin.2020.02.043. 67. P. Gruber, L. Remonda. Device profile of different paclitaxel-coated balloons: Neuro Elutax SV, Elutax ‘3’ Neuro and SeQuent Please NEO for the treatment of symptomatic intracranial high-grade stenosis: overview of their feasibility and safety. Expert Rev. Med. Devices. 17 (2020) 87–92. doi:10.1080/17434440.2020.1719829. 68. B. Cortese, P. Silva Orrego, P. Agostoni, D. Buccheri, D. Piraino, G. Andolina, R.G. Seregni. Effect of drug-coated balloons in native coronary artery disease left with a dissection. JACC Cardiovasc. Interv. 8 (2015) 2003–2009. doi:10.1016/j.jcin.2015.08.029. 69. M. Kimura, J. Shiraishi, N. Ikemura, Y. Matsubara, M. Hyogo, T. Sawada. Proximal balloon occlusion to prevent downstream embolization and thus reduce systemic adverse effects of drug-coated balloons. Cardiovasc. Interv. Ther. 35 (2020) 306–307. doi:10.1007/s12928-019-00595-9. 70. J. Chlupác, E. Filová, L. Bačáková. Blood vessel replacement: 50 years of development and tissue engineering paradigms in vascular surgery. Physiol. Res. 58 (2009) 119–140. 71. A.B. Voorhees, A. Jaretzki, A.H. Blakemore. The use of tubes constructed from vinyon “N” cloth in bridging arterial defects. Ann. Surg. 135 (1952) 332–336. doi:10.1097/ 00000658-195203000-00006. 72. J.D. Kakisis, C.D. Liapis, C. Breuer, B.E. Sumpio. Artificial blood vessel: The Holy Grail of peripheral vascular surgery. J. Vasc. Surg. 41 (2005) 349–354. doi:10.1016/j. jvs.2004.12.026.
Cardiovascular Therapeutic Devices
73. D. Wang, Y. Xu, Q. Li, L.S. Turng. Artificial small-diameter blood vessels: Materials. fabrication, surface modification, mechanical properties, and bioactive functionalities. J. Mater. Chem. B. 8 (2020) 1801–1822. doi:10.1039/c9tb01849b. 74. H.J. Chung, T.G. Park. Surface engineered and drug releasing pre-fabricated scaffolds for tissue engineering. Adv. Drug Deliv. Rev. 59 (2007) 249–262. doi:10.1016/j. addr.2007.03.015. 75. Z. Wang, S.M. Mithieux, A.S. Weiss. Fabrication techniques for vascular and vascularized tissue engineering. Adv. Healthc. Mater. 8 (2019) 1–26. doi:10.1002/adhm. 201900742. 76. J. Fu, M. Wang, I. De Vlaminck, Y. Wang. Thick PCL fibers improving host remodeling of PGS-PCL composite grafts implanted in rat common carotid arteries. Small. 16 (2020) 2004133. doi:10.1002/smll.202004133. 77. C.E.T. Stowell, X. Li, M.H. Matsunaga, C.B. Cockreham, K.M. Kelly, J. Cheetham, E. Tzeng, Y. Wang. Resorbable vascular grafts show rapid cellularization and degradation in the ovine carotid. J. Tissue Eng. Regen. Med. 14 (2020) 1673–1684. doi:10.1002/ term.3128. 78. J.C. Zbinden, K.M. Blum, A.G. Berman, A.B. Ramachandra, J.M. Szafron, K.E. Kerr, J.L. Anderson, G.S. Sangha, C.C. Earl, N.R. Nigh, G.J.M. Mirhaidari, J.W. Reinhardt, Y.C. Chang, T. Yi, R. Smalley, P.D. Gabriele, J.J. Harris, J.D. Humphrey, C.J. Goergen, C.K. Breuer. Effects of braiding parameters on tissue engineered vascular graft development. Adv. Healthc. Mater. 2001093 (2020) 1–12. doi:10.1002/adhm.202001093. 79. A. Ranjbarzadeh-Dibazar, J. Barzin, P. Shokrollahi. Microstructure crystalline domains disorder critically controls formation of nano-porous/long fibrillar morphology of ePTFE membranes. Polymer (Guildf) 121 (2017) 75–87. doi:10.1016/j.polymer. 2017.06.003. 80. M. Tozzi, M. Franchin, G. Ietto, G. Soldini, G. Carcano, P. Castelli, G. Piffaretti. Initial experience with the Gore® Acuseal graft for prosthetic vascular access. J. Vasc. Access. 15 (2014) 385–390. doi:10.5301/jva.5000276. 81. J. Li, Y. Long, F. Yang, H. Wei, Z. Zhang, Y. Wang, J. Wang, C. Li, C. Carlos, Y. Dong, Y. Wu, W. Cai, X. Wang. Multifunctional artificial artery from direct 3D printing with built-in ferroelectricity and tissue-matching modulus for real-time sensing and occlusion monitoring. Adv. Funct. Mater. 30 (2020). doi:10.1002/adfm.202002868. 82. D.J. Lyman, W.M. Muir, I.J. Lee. The effect of chemical structure and surface properties of polymers on the coagulation of blood. I. Surface free energy effects. Trans. Am. Soc. Artif. Intern. Organs. 11 (1965) 301–306. doi:10.1097/00002480-196504000-00056. 83. S. Srinivasan, P.N. Sawyer. Role of surface charge of the blood vessel wall, blood cells, and prosthetic materials in intravascular thrombosis. J. Colloid Interface Sci. 32 (1970) 456–463. doi:10.1016/0021-9797(70)90131-1. 84. A. Takahara., J. Ichi Tashita, T. Kajiyama, M. Takayanagi, W.J. MacKnight. Microphase separated structure, surface composition and blood compatibility of segmented poly(urethaneureas) with various soft segment components. Polymer (Guildf). 26 (1985) 987–996. doi:10.1016/0032-3861(85)90218-6. 85. S.P. Hoerstrup, I. Cummings, M. Lachat, F.J. Schoen, R. Jenni, S. Leschka, S. Neuenschwander, D. Schmidt, A. Mol, C. Günter, M. Gössi, M. Genoni, G. Zund. Func tional growth in tissue-engineered living, vascular grafts: Follow-up at 100 weeks in a large animal model. Circulation. 114 (2006) 159–166. doi:10.1161/CIRCULATIONAHA. 105.001172. 86. B. Nasiri, S. Row, R.J. Smith, D.D. Swartz, S.T. Andreadis. Cell-free vascular grafts that grow with the host. Adv. Funct. Mater. 30 (2020) 1–11. doi:10.1002/adfm.202005769. 87. J. DelBianco, S. Steerman, D. Dexter, S. Ahanchi, G. Stokes, S. Ongstad, O. Powell, N. Parikh, J. Panneton. Early-access upper extremity grafts offer no benefit over standard grafts in hemodialysis access. J. Vasc. Surg. 65 (2017) e6. doi:10.1016/j.jvs.2016.12.037.
Biomaterials and Materials for Medicine
88. S.P. Schmidt, T.J. Hunter, M. Hirko, T.A. Belden, M. Michelle Evancho, W. V. Sharp, D.L. Donovan. Small-diameter vascular prostheses: Two designs of PTFE and endothelial cell-seeded and nonseeded Dacron. J. Vasc. Surg. 2 (1985) 292–297. doi:10.1016/ 0741-5214(85)90068-0. 89. R.I. Mehta, A.K. Mukherjee, T.D. Patterson, M.C. Fishbein. Pathology of explanted polytetrafluoroethylene vascular grafts. Cardiovasc. Pathol. 20 (2011) 213–221. doi:10. 1016/j.carpath.2010.06.005. 90. S. de Valence, J.C. Tille, D. Mugnai, W. Mrowczynski, R. Gurny, M. Möller, B.H. Walpoth. Long term performance of polycaprolactone vascular grafts in a rat abdominal aorta replacement model. Biomaterials. 33 (2012) 38–47. doi:10.1016/j. biomaterials.2011.09.024. 91. C. Wang, L. Cen, S. Yin, Q. Liu, W. Liu, Y. Cao, L. Cui. A small diameter elastic blood vessel wall prepared under pulsatile conditions from polyglycolic acid mesh and smooth muscle cells differentiated from adipose-derived stem cells. Biomaterials. 31 (2010) 621–630. doi:10.1016/j.biomaterials.2009.09.086. 92. Yang Hongjun, H. Xu. W. Xu, W. Wang, O.Y. Chenxi. Preparation of small-diameter artificial blood vessel with a biomimic structure. In: 3rd Natl. Conf. Vasc. Surg. Tissue Engineering, Wuhan, China, 2008, issued online 2010:23–27. 93. Z. Wang, C. Liu, Y. Xiao, X. Gu, Y. Xu, N. Dong, S. Zhang, Q. Qin, J. Wang. Remodeling of a cell-free vascular graft with nanolamellar intima into a neovessel. ACS Nano. 13 (2019) 10576–10586. doi:10.1021/acsnano.9b04704. 94. H. Yamanaka, T. Yamaoka, A. Mahara, N. Morimoto, S. Suzuki. Tissue-engineered submillimeter-diameter vascular grafts for free flap survival in rat model. Biomaterials. 179 (2018) 156–163. doi:10.1016/j.biomaterials.2018.06.022. 95. L. Xu, M. Varkey, A. Jorgensen, J. Ju, Q. Jin, J.H. Park, Y. Fu, G. Zhang, D. Ke, W. Zhao, R. Hou, A. Atala. Bioprinting small diameter blood vessel constructs with an endothelial and smooth muscle cell bilayer in a single step. Biofabrication. 12 (2020). doi:10.1088/1758-5090/aba2b6. 96. K. Yamamoto, Y. Nogimori, H. Imamura, J. Ando. Shear stress activates mitochondrial oxidative phosphorylation by reducing plasma membrane cholesterol in vascular endothelial cells. Proc. Natl. Acad. Sci. 117 (2020) 33660–33667. doi:10.1073/pnas.2014029117. 97. L.E. Niklason, J.H. Lawson. Bioengineered human blood vessels. Science. 370 (2020) eaaw8682. doi:10.1126/science.aaw8682. 98. B. Wiatrak, Z. Rybak. History, present and future of biomaterials used for artificial heart valves. Polim. Med. 43(3) (2014) 183–189. PMID:24377185. 99. B.O. D.J. Wheatley, G.M. Bernacca. Cardiac surgery: Biomaterials. in: Encyclopedia of Materials: Science and Technology, K.H. Jürgen Buschow, R.W. Cahn, M.C. Flemings, B. Ilschner, E.J. Kramer, S. Mahajan, P. Veyssière, Elsevier, Oxford, UK, 2001: 999–1003. 100. R. Major, M. Gonsior, M. Sanak, M. Kot, R. Kustosz, J.M. Lackner. Surface modification of metallic materials designed for a new generation of artificial heart valves. Int. J. Artif. Organs. 41 (2018) 854–866. doi:10.1177/0391398818794064. 101. D.L. Bark, A. Yousefi, M. Forleo, A. Vaesken, F. Heim, L.P. Dasi. Reynolds shear stress for textile prosthetic heart valves in relation to fabric design. J. Mech. Behav. Biomed. Mater. 60 (2016) 280–287. doi:10.1016/j.jmbbm.2016.01.016. 102. A. Vaesken, F. Heim, N. Chakfe. Fiber heart valve prosthesis: Influence of the fabric construction parameters on the valve fatigue performances. J. Mech. Behav. Biomed. Mater. 40 (2014) 69–74. doi:10.1016/j.jmbbm.2014.08.015. 103. F. Heim, B. Durand, N. Chakfe. Textile heartvalve prosthesis: Manufacturing process and prototype performances. Text. Res. J. 12 (2008) 1124–1131. doi:10.1177/ 0040517508092007.
Cardiovascular Therapeutic Devices
104. F. Piatti, F. Sturla, G. Marom, J. Sheriff, T.E. Claiborne, M.J. Slepian, A. Redaelli, D. Bluestein. Hemodynamic and thrombogenic analysis of a trileaflet polymeric valve using a fluid-structure interaction approach. J. Biomech. 48 (2015) 3650–3658. doi:10.1016/ j.jbiomech.2015.08.009. 105. H. Tashiro, M.B. Popović, I. Dobrev, Y. Terasawa. Artificial organs. tissues, and support systems, in: Biomechatronics, mARKO B. POPOVIC (Ed.), Elsevier, 2019: pp. 175–199. doi:10.1016/B978-0-12-812939-5.00007-0. 106. M.F. O’Brien, D.C. McGiffin, E.G. Stafford, M.A.H. Gardner, P.F. Pohlner, G.J. McLachlan, K. Gall, S. Smith, E. Murphy. Allograft aortic valve replacement: Long-term comparative clinical analysis of the viable cryopreserved and antibiotic 4°C stored valves. J. Card. Surg. 6 (1991) 534–543. doi:10.1111/jocs.1991.6.4s.534. 107. P. Palka, S. Harrocks, A. Lange, D.J. Burstow, M.F. O’Brien. Primary aortic valve replacement with cryopreserved aortic allograft: An echocardiographic follow-up study of 570 patients. Circulation. 105 (2002) 61–66. doi:10.1161/hc0102.101357. 108. J.C. Witten, E. Durbak, P.L. Houghtaling, S. Unai, E.E. Roselli, F.G. Bakaeen, D.R. Johnston, L.G. Svensson, W. Jaber, E.H. Blackstone, G.B. Pettersson. Performance and durability of cryopreserved allograft aortic valve replacements. Ann. Thorac. Surg. (2020). doi:10.1016/j.athoracsur.2020.07.033. In Press Journal Pre-Proof. 109. F. Nappi, A. Nenna, T. Petitti, C. Spadaccio, I. Gambardella, M. Lusini, M. Chello, C. Acar. Long-term outcome of cryopreserved allograft for aortic valve replacement. J. Thorac. Cardiovasc. Surg. 156 (2018) 1357–1365. doi:10.1016/j.jtcvs.2018.04.040. 110. M.B. Forman, J.B. Atkinson, J.A. Wolfe, R.A. Hopkins. Non-bacterial thrombotic endocarditis in an adult 14 months after cryopreserved aortic allograft valve implantation. J. Heart Valve Dis. 16 (2007) 410–416. PMID: 17702367. 111. J.R. Doty, J.D. Salazar, J.R. Liddicoat, J.H. Flores, D.B. Doty, R.S. Mitchell, V.A. Starnes, F. Khouqeer. Aortic valve replacement with cryopreserved aortic allograft: Ten-year experience. J. Thorac. Cardiovasc. Surg. 115 (1998) 371–380. doi:10.1016/ S0022-5223(98)70281-8. 112. M. Ruzmetov, J.J. Shah, D.M. Geiss, R.S. Fortuna. Decellularized versus standard cryopreserved valve allografts for right ventricular outflow tract reconstruction: A singleinstitution comparison. J. Thorac. Cardiovasc. Surg. 143 (2012) 543–549. doi:10.1016/j. jtcvs.2011.12.032. 113. K. Bando. A proposal for prospective late outcome analysis of decellularized aortic valves. J. Thorac. Cardiovasc. Surg. 152 (2016) 1202–1203. doi:10.1016/j.jtcvs. 2016.04.087. 114. M.R.K. Helder, N.T. Kouchoukos, K. Zehr, J.A. Dearani, J.J. Maleszewski, C. Leduc, C.N. Heins, H. V. Schaff. Late durability of decellularized allografts for aortic valve replacement: A word of caution. J. Thorac. Cardiovasc. Surg. 152 (2016) 1197–1199. doi:10.1016/j.jtcvs.2016.03.050. 115. M. Vrandecic, B. Gontijo, F. Fantini, C. Acar. Homograft replacement of the mitral valve. J. Thorac. Cardiovasc. Surg. 112 (1996) 1678–1679. doi:10.1016/S0022-5223(96)70032-6. 116. R.A. Hopkins, A. Reyes, D.A. Imperato, G.A. Carpenter, J.L. Myers, K.A. Murphy. Ventricular outflow tract reconstructions with cryopreserved cardiac valve homografts: A single surgeon’s 10-year experience. Ann. Surg. 223 (1996) 544–553. doi:10.1097/ 00000658-199605000-00010. 117. W. Flameng, G. De Visscher, L. Mesure, H. Hermans, R. Jashari, B. Meuris. Coating with fibronectin and stromal cell-derived factor-1α of decellularized homografts used for right ventricular outflow tract reconstruction eliminates immune response-related degeneration. J. Thorac. Cardiovasc. Surg. 147 (2014) 1398–1404. doi:10.1016/j. jtcvs.2013.06.022.
Biomaterials and Materials for Medicine
118. M.Y. Emmert, B. Weber, L. Behr, T. Frauenfelder, C.E. Brokopp, J. Grnenfelder, V. Falk, S.P. Hoerstrup. Transapical aortic implantation of autologous marrow stromal cell-based tissue-engineered heart valves: First experiences in the systemic circulation. JACC Cardiovasc. Interv. 4 (2011) 822–823. doi:10.1016/j.jcin.2011.02.020. 119. C. Lueders, B. Jastram, R. Hetzer, H. Schwandt. Rapid manufacturing techniques for the tissue engineering of human heart valves. Eur. J. Cardio-Thoracic Surg. 46 (2014) 593–601. doi:10.1093/ejcts/ezt510. 120. J.M. Reimer, Z.H. Syedain, B.H.T. Haynie, R.T. Tranquillo. Pediatric tubular pulmonary heart valve from decellularized engineered tissue tubes. Biomaterials. 62 (2015) 88–94. doi:10.1016/j.biomaterials.2015.05.009. 121. L.A. Hockaday, K.H. Kang, N.W. Colangelo, P.Y.C. Cheung, B. Duan, E. Malone, J. Wu, L.N. Girardi, L.J. Bonassar, H. Lipson, C.C. Chu, J.T. Butcher. Rapid 3D printing of anatomically accurate and mechanically heterogeneous aortic valve hydrogel scaffolds. Biofabrication. 4 (2012) 035005. doi:10.1088/1758–5082/4/3/035005. 122. R.A. Hopkins, A.A. Bert, S.L. Hilbert, R.W. Quinn, K.M. Brasky, W.B. Drake, G.K. Lofland. Bioengineered human and allogeneic pulmonary valve conduits chronically implanted orthotopically in baboons: Hemodynamic performance and immunologic consequences. J. Thorac. Cardiovasc. Surg. 145 (2013) 1098–1107. doi:10.1016/j.jtcvs.2012.06.024. 123. T.C. Flanagan, C. Cornelissen, S. Koch, B. Tschoeke, J.S. Sachweh, T. Schmitz-Rode, S. Jockenhoevel. The in vitro development of autologous fibrin-based tissue-engineered heart valves through optimised dynamic conditioning. Biomaterials. 28 (2007) 3388– 3397. doi:10.1016/j.biomaterials.2007.04.012. 124. S. Sant, D. Iyer, A.K. Gaharwar, A. Patel, A. Khademhosseini. Effect of biodegradation and de novo matrix synthesis on the mechanical properties of valvular interstitial cell-seeded polyglycerol sebacate-polycaprolactone scaffolds. Acta Biomater. 9 (2013) 5963–5973. doi:10.1016/j.actbio.2012.11.014. 125. M. Weber, I. Gonzalez De Torre, R. Moreira, J. Frese, C. Oedekoven, M. Alonso, C.J. Rodriguez Cabello, S. Jockenhoevel, P. Mela. Multiple-step injection molding for fibrin-based tissue-engineered heart valves. Tissue Eng. - Part C Methods. 21 (2015) 832–840. doi:10.1089/ten.tec.2014.0396. 126. N. Masoumi, N. Annabi, A. Assmann, B.L. Larson, J. Hjortnaes, N. Alemdar, M. Kharaziha, K.B. Manning, J.E. Mayer, A. Khademhosseini. Tri-layered elastomeric scaffolds for engineering heart valve leaflets. Biomaterials. 35 (2014) 7774–7785. doi:10.1016/j. biomaterials.2014.04.039. 127. N. Masoumi, A. Jean, J.T. Zugates, K.L. Johnson, G.C. Engelmayr. Laser microfabricated poly(glycerol sebacate) scaffolds for heart valve tissue engineering. J. Biomed. Mater. Res. - Part A 101 (2013) 104–114. doi:10.1002/jbm.a.34305. 128. P.E. Dijkman, A. Driessen-Mol, L. Frese, S.P. Hoerstrup, F.P.T. Baaijens. Decellularized homologous tissue-engineered heart valves as off-the-shelf alternatives to xeno- and homografts. Biomaterials. 33 (2012) 4545–4554. doi:10.1016/j.biomaterials.2012.03.015. 129. K. MacIntyre, S. Capewell, S. Stewart, J.W.T. Chalmers, J. Boyd, A. Finlayson, A. Redpath, J.P. Pell, J.J.V. McMurray. Evidence of improving prognosis in heart failure: Trends in case fatality in 66 547 patients hospitalized between 1986 and 1995. Circulation 102 (2000) 1126–1131. doi:10.1161/01.CIR.102.10.1126. 130. S.N. Doost, L. Zhong, Y.S. Morsi. Ventricular assist devices: Current state and challenges. J. Med. Devices, Trans. ASME. 11 (2017) 040801. doi:10.1115/1.4037258. 131. G. Luraghi, W. Wu, H. De Castilla, J.F. Rodriguez Matas, G. Dubini, P. Dubuis, M. Grimmé, F. Migliavacca. Numerical approach to study the behavior of an artificial ventricle: Fluid–structure interaction followed by fluid dynamics with moving boundaries. Artif. Organs. 42 (2018) E315–E324. doi:10.1111/aor.13316.
Cardiovascular Therapeutic Devices
132. B. Pelletier, S. Spiliopoulos, T. Finocchiaro, F. Graef, K. Kuipers, M. Laumen, D. Guersoy, U. Steinseifer, R. Koerfer, G. Tenderich. System overview of the fully implantable destination therapy--ReinHeart-total artificial heart. Eur. J. Cardiothorac. Surg. 40 (2015) 80–86. doi:10.1093/ejcts/ezu321. 133. J.A. Cook, K.B. Shah, M.A. Quader, R.H. Cooke, V. Kasirajan, K.K. Rao, M.C. Smallfield, I. Tchoukina, D.G. Tang. The total artificial heart. J. Thorac. Dis. 7 (2015) 2172–2180. doi:10.3978/j.issn.2072-1439.2015.10.70. 134. J.G. Copeland, R.G. Smith, F.A. Arabia, P.E. Nolan, G.K. Sethi, P.H. Tsau, D. McClellan, M.J. Slepian. Cardiac Replacement with a total artificial heart as a bridge to transplantation. N. Engl. J. Med. 351 (2004), 859–867. doi:10.1056/nejmoa040186. 135. G. Gerosa, S. Scuri, L. Iop, G. Torregrossa. Present and future perspectives on total artificial hearts. Ann. Cardiothorac. Surg. 3 (2014) 595–602. doi:10.3978/j.issn.2225319X.2014.09.05. 136. S.D. Gregory, J. Zwischenberger, D.F. Wang, S. Liao, M. Slaughter. Chapter 18Cannula design, in: Mechanical Circulatory and Respiratory Support, S.D. Gregory, M.C. Stevens, J.F. Fraser (Eds.), Academic Press, 2017: pp. 567–596. doi:10.1016/ c2016-0-00501-6. 137. M.E. Stone, J. Hinchey. Mechanical assist devices for heart failure, in: Kaplan’s Essentials Cardiac Anesthesia, 2nd ed., J.A. Kaplan (Ed.), Elsevier, 2018: pp. 51–583. doi:10.1016/B978-0-323-49798-5.00022-X. 138. A. Carpentier, C. Latrémouille, B. Cholley, D.M. Smadja, J.C. Roussel, E. Boissier, J.N. Trochu, J.P. Gueffet, M. Treillot, P. Bizouarn, D. Méléard, M.F. Boughenou, O. Ponzio, M. Grimmé, A. Capel, P. Jansen, A. Hagège, M. Desnos, J.N. Fabiani, D. Duveau. First clinical use of a bioprosthetic total artificial heart: Report of two cases. Lancet. 386 (2015) 1556–1563. doi:10.1016/S0140-6736(15)60511-6. 139. P. Jansen, W. van Oeveren, A. Capel, A. Carpentier. In vitro haemocompatibility of a novel bioprosthetic total artificial heart. Eur. J. Cardio-Thoracic Surg. 41 (2012) e166– e172. doi:10.1093/ejcts/ezs187. 140. U. Richez, H. De Castilla, C.L. Guerin, N. Gendron, G. Luraghi, M. Grimme, W. Wu, M. Taverna, P. Jansen, C. Latremouille, F. Migliavacca, G. Dubini, A. Capel, A. Carpentier, D.M. Smadja. Hemocompatibility and safety of the carmat total artifical heart hybrid membrane. Heliyon. 5 (2019) e02914. doi:10.1016/j.heliyon.2019.e02914. 141. D.M. Smadja, B. Saubaméa, S. Susen, M. Kindo, P. Bruneval, E. Van Belle, P. Jansen, J.C. Roussel, C. Latrémouille, A. Carpentier. Bioprosthetic total artificial heart induces a profile of acquired hemocompatibility with membranes recellularization. J. Am. Coll. Cardiol. 70 (2017) 404–406. doi:10.1016/j.jacc.2017.05.021. 142. D.M. Smadja, R. Chocron, E. Rossi, B. Poitier, Y. Pya, M. Bekbossynova, C. Peronino, J. Rancic, J.C. Roussel, M. Kindo, N. Gendron, L. Migliozzi, A. Capel, J.C. Perles, P. Gaussem, P. Ivak, P. Jansen, C. Girard, A. Carpentier, C. Latremouille, C. Guerin, I. Netuka. Autoregulation of pulsatile bioprosthetic total artificial heart is involved in endothelial homeostasis preservation. Thromb. Haemost. (2020) s-0040–1713751. doi:10.1055/s-0040-1713751. 143. M. Diedrich, S. Hildebrand, M.K. Lommel, T. Finocchiaro, E. Cuenca, H. De Ben, T. Schmitz-Rode, U. Steinseifer, S. Jansen. Experimental investigation of right-left flow balance concepts for a total artificial heart. Artif. Organs. (2020) 13830. doi:10.1111/ aor.13830. 144. J.K. Kirklin, F.D. Pagani, R.L. Kormos, L.W. Stevenson, E.D. Blume, S.L. Myers, M.A. Miller, J.T. Baldwin, J.B. Young, D.C. Naftel. Eighth annual INTERMACS report: Special focus on framing the impact of adverse events. J. Hear. Lung Transplant. (2017) S105324981731896X. doi:10.1016/j.healun.2017.07.005.
Biomaterials and Materials for Medicine
145. L.E. Rodriguez, E.E. Suarez, M. Loebe, B.A. Bruckner. Ventricular assist devices (VAD) therapy: New technology, new hope? Methodist Debakey Cardiovasc. J. 9 (2013) 32–37. doi:10.14797/mdcj-9-1-32. 146. J. Wohlschlaeger, K.J. Schmitz, C. Schmid, K.W. Schmid, P. Keul, A. Takeda, S. Weis, B. Levkau, H.A. Baba. Reverse remodeling following insertion of left ventricular assist devices (LVAD): A review of the morphological and molecular changes. Cardiovasc. Res. 68 (2005) 376–386. doi:10.1016/j.cardiores.2005.06.030. 147. S.R. Wilson, M.M. Givertz, G.C. Stewart, G.H. Mudge. Ventricular assist devices. The challenges of outpatient management. J. Am. Coll. Cardiol. 54 (2009) 1647–1659. doi:10.1016/j.jacc.2009.06.035. 148. B.C. Blaxall, B.M. Tschannen-Moran, C.A. Milano, W.J. Koch. Differential gene expression and genomic patient stratification following Left Ventricular Assist Device support. J. Am. Coll. Cardiol. 41 (2003) 1096–1106. doi:10.1016/S0735-1097(03)00043-3. 149. N. Morici, M. Varrenti, D. Brunelli, E. Perna, M. Cipriani, E. Ammirati, M. Frigerio, M. Cattaneo, F. Oliva. Antithrombotic therapy in ventricular assist device (VAD) management: From ancient beliefs to updated evidence. A narrative review. IJC Hear. Vasc. 20 (2018) 20–26. doi:10.1016/j.ijcha.2018.06.005. 150. C. Murphy, H. Zafar, F. Sharif. An updated review of cardiac devices in heart failure. Ir. J. Med. Sci. 186 (2017) 909–919. doi:10.1007/s11845-017-1597-9. 151. J. Garbade, H.B. Bittner, M.J. Barten, F.W. Mohr. Current trends in implantable left ventricular assist devices. Cardiol. Res. Pract. 17 (2011) 290561. doi:10.4061/2011/290561. 152. S. Agarwal, K.M. High. Newer-generation ventricular assist devices. Best Pract. Res. Clin. Anaesthesiol. 26 (2012) 117–130. doi:10.1016/j.bpa.2012.01.003. 153. T. Wu, A.W. Khir, M. Kütting, X. Du, H. Lin, Y. Zhu, P.L. Hsu, A review of implantable pulsatile blood pumps: Engineering perspectives. Int. J. Artif. Organs. (2020) 039139882090247. doi:10.1177/0391398820902470.
Vascular Patches: Past and Future, Problems, and Solutions Hualong Bai First Affiliated Hospital of Zhengzhou University Key Vascular Physiology and Applied Research Laboratory of Zhengzhou City
Yanhua Xu The First Affiliated Hospital of Zhengzhou University
Hao He and Xin Li Central South University
Chang Shu Central South University Chinese Academy of Medical Sciences and Peking Union Medical College
Jingan Li Zhengzhou University
Quancheng Kan The First Affiliated Hospital of Zhengzhou University Zhengzhou University
Alan Dardik Yale School of Medicine
CONTENTS 2.1 2.2 2.3 2.4 2.5
Animal Model.................................................................................................. 36 Patch Materials................................................................................................ 37 Patch Healing After Implantation................................................................... 39 Tissue-Engineered Vascular Patches............................................................... 41 Complications of Patches................................................................................. 42
Biomaterials and Materials for Medicine
2.6 Future Research Directions.............................................................................44 Acknowledgements...................................................................................................44 Disclosure.................................................................................................................44 References.................................................................................................................44
2.1 ANIMAL MODEL To study neointimal hyperplasia after patch implantation in both arteries and veins, Bai et al. developed a rat model of patch angioplasty that can be used in either a vein (inferior vena cava, (IVC) venoplasty) or an artery (abdominal aorta, arterioplasty); the diameter of the vessels can range widely from less than 1 mm to larger than 2 mm . The technical details are described briefly. Microsurgical procedures are performed aseptically using a dissecting microscope. The infrarenal aorta or IVC is exposed below the level of the renal arteries, and then clamped proximally and distally. A longitudinal 3-mm arteriotomy or venotomy is made on the anterior wall of the aorta or IVC. The arteriotomy or venotomy is closed with a patch using continuous 10-0 nylon sutures, and the vessel clamps are removed. The abdomen is closed, and the rat is allowed to recover; no immunosuppressive agents or heparin are administered at any time. Because patch angioplasty is widely used in human patients after arteriotomies in medium-diameter (4–8 mm) vessels, such as after carotid artery endarterectomy (Figure 2.1a and b), our group also applied the patch angioplasty model to the rat carotid artery (Figure 2.1c). Although this model variation uses an arteriotomy on the common carotid artery that does not include the internal carotid artery, the hemodynamics in this vessel may still be a reasonable model of the hemodynamics within the carotid artery of human patients. Elastin staining shows the patch incorporated to the native carotid artery and a neointima formed on day 14 (Figure 2.2). Compared to other models, the rat aortic and IVC patch angioplasty models have some merits: first, this model does not need to replace a segment of aorta or IVC, and thus is technically easier to perform compared to interposition grafts
FIGURE 2.1 Photographs showing vascular patches in human and rat carotid arteries. (a) Illustration showing placement of a patch in the human carotid bifurcation (Adobe illustrator CS). (b) Intraoperative photograph showing patch angioplasty in a human carotid artery after carotid artery endarterectomy. (c) Rat carotid artery patch arterioplasty; scale bar, 1 mm. Arrows show the patches.
FIGURE 2.2 Verhoeff’s Van Gieson staining of a rat carotid artery patch angioplasty; the patch is decellularized rat carotid artery. Scale bar, 1 mm or 100 μm; note the ratio of the width of patch to the diameter of the vessel is approximately 3. Dashed line demarcating the carotid artery patch and neointima.
models. Additionally, reduced surgical time can decrease the rate of lower limb ischemic complications. Second, compared to some other models, this model has a rapid thick neointimal formation [1,2]. Neointimal cells are found on the patch as early as day 3, and neointima is formed on day 7. Because different patch materials can influence the thickness of the neointima, different thickness of neointima is found after day 7 [3–6].
2.2 PATCH MATERIALS Dacron and expanded polytetrafluoroethylene (ePTFE) have been used therapeutically in human patients for more than half a century, and these materials are still widely used in vascular procedures today. Whinfield and Dickinson developed the polyester fabric Dacron in 1941, and it was first used in humans as an aortic graft by Dr DeBakey in 1953 . Dacron grafts can be knitted or woven; knitted grafts have better compliance but they also have larger pores that require preclotting to prevent bleeding after implantation. At present, knitted Dacron grafts are coated with albumin to prevent leakage. Dacron is estimated to last more than 30 years after implantation, but these grafts have a high risk of dilation . Dacron is commonly used as a large-diameter graft in aortic and lower-extremity bypass surgery , and can be used in the rat patch model (Figure 2.3a). Matsumoto and colleagues introduced ePTFE in 1973, and Gore expanded the use of this material; ePTFE was found to be suitable for vascular replacement . ePTFE grafts are compliant, easy to suture, and do not need to be preclotted compared to knitted Dacron grafts. ePTFE does show some suture line bleeding, and it can also induce a foreign body reaction, have a tendency toward thrombosis, and can have an increased risk of infection . ePTFE can be used in the rat patch model and show increased time to hemostasis after aortic arterioplasty (Figure 2.3b). Compared to synthetic vascular materials, decellularized tissues have a similar extracellular matrix and similar structural architecture as native vessels, but with reduced immunogenicity [5,12,13]. The pericardium is commonly used as a patch after arteriotomy during cardiovascular surgery. Compared to Dacron and ePTFE, pericardial patches have several advantages, including superior biocompatibility, easy handling, and less suture line bleeding. Li et al. showed a similar healing process of
Biomaterials and Materials for Medicine
FIGURE 2.3 Patch angioplasty with different materials. (a) Polyester patch venoplasty and arterioplasty ruler marks 1 mm. (b) Rat IVC ePTFE patch venoplasty, ruler marks 1 mm. (c) Verhoeff’s Van Gieson staining showing the rat autologous jugular vein and carotid artery patch angioplasty at day 14; scale bar, 1 mm.
bovine and porcine pericardial patch using the rat aortic arterioplasty model . Bai et al. showed some similarities and differences in healing after arterioplasty and venoplasty in rats using pericardial patches . Dacron, ePTFE, and pericardial patches show some compliance mismatch with native vessels [15–17]. To determine if decellularized vessels can minimize the compliance mismatch when used as patches, we examined decellularized human saphenous vein patches (2 mm × 3 mm) implanted to the rat aorta and IVC . The healing process is similar to that of pericardial patches, despite the human saphenous vein patch being much thicker compared to the rat aorta. We similarly tested decellularized rat thoracic aorta as a patch ; the rat thoracic aorta and abdominal aorta have a similar thickness (150 ± 3 vs. 156 ± 4 μm; p = 0.2914; t-test) and can be successfully used as a patch material . In addition to the commonly used prosthetic and biological vascular materials, autologous materials are also widely used in vascular surgeries. Because autologous vascular grafts have the lowest immunoreaction and the best patency rate of all vascular grafts, we examined autologous carotid artery and jugular vein patches in the rat arterioplasty and venoplasty models; both grafts showed a similar healing process, although the jugular vein dilated as early as day 14 after implantation into the rat aorta, consistent with its high compliance (Figure 2.3c) .
Other materials have been tested in the patch angioplasty model. One group showed that sugarcane biopolymer membrane can be used as a patch in femoral vein angioplasty in dogs; they showed there were no cases of infection, rupture, pseudoaneurysm formation, or thrombosis. There was a chronic inflammatory reaction with lymphocytes, neutrophils, and fibrosis in the outer surface of the patches. The authors concluded that sugarcane biopolymer membrane is easily synthesized with a low cost of production and can be successfully used in femoral vein patch angioplasty . However, whether this material is permanent or is resorbable in vivo is not clear and thus longer-term studies are needed. Another group examined the peritoneum-fascia patch and found similar clotresistant properties as polyester with superior mechanical strength compared with the pericardial patch . Although this group used a peritoneum patch to repair an infected aortic stump successfully and reported this case , no further research was reported. However, this shows the promising application of autologous modified tissue to be used as a vascular substitute. Glutaraldehyde fixation cross-links proteins in xenogeneic tissues, such as bovine pericardium, minimizing immune rejection and sterilizing the tissue; however, fixation may also compromise the regenerative potential of the resultant biomaterial [21,22]. One group compared SDS decellularization and glutaraldehyde fixation and showed the importance of residual antigenicity and extracellular matrix architecture preservation in modulating recipient immune and regenerative responses toward xenogeneic biomaterials . Small intestinal submucosa (SIS) is a cell-free collagen matrix derived from porcine small intestine that has been used in wound healing , as well as a vascular patch. SIS (CorMatrix) showed no short-term adverse events when used as an aortic interposition tube graft, but there was a high rate of neointimal hyperplasia with significant stenosis in low-pressure, small-diameter conduits . Clinical results using SIS have not been consistent. One group found complete incorporation and no false aneurysm formation when compared with PTFE . Jacobsen et al. reported porcine SIS patches may be an appropriate tissue choice for Norwood procedures . However, McCready et al. reported 7 of 76 patients developed pseudoaneurysms in less than 10 weeks . Madden et al. reported using a small intestine submucosa patch after carotid artery endarterectomy and suggested further studies . These different reports show the complex development of new vascular materials and suggest that well-performed, adequately powered, multi-centered clinical trials are needed.
2.3 PATCH HEALING AFTER IMPLANTATION After implantation of prosthetics, rapid reendothelialization is critical to prevent thrombus formation. Sauvage et al. compared reendothelialization in humans, dogs, pigs, calves, and baboons, and reported that humans and dogs are limited in their ability to develop pannus ingrowth from the anastomoses, whereas pigs, calves, and baboons heal very rapidly. Healing of porous prostheses is assisted by a filamentous external surface, particularly in humans and dogs . This seminal research showed the importance of neointimal reendothelialization after prosthetic implantation in vascular surgeries.
Biomaterials and Materials for Medicine
Both patch arterioplasty and venoplasty share a similar healing process; patches in the rat model show rapid reendothelialization as early as day 7, with CD34 and VEGFR2 dual-positive cells, that is, endothelial progenitor cells (EPC), located on the luminal side of the neointima . EPC also display markers such as vWF and CD31 [2,31]. Below the EPC are other cell types, including SMCs, macrophages, leukocytes, mesenchymal cells, lymphocytes, CD90-positive cells, nestin-positive cells, and other cells that all potentially contribute to the neointimal formation, similar to the human process . Among these cells, SMCs and macrophages play an important role in neointimal hyperplasia; we found that one-third of the SMCs  and half of the macrophages were PCNA- or Ki67-positive (Figure 2.4). In addition, there were more PCNA- and CD68-positive cells in the venous patches compared to arterial patches. These data suggest that both SMC and macrophages were proliferating and could be targets of anti-proliferation treatment. Although statin drugs are commonly used for vascular disease, whether statins influence neointimal formation or arterial endothelial cell infiltration after patch angioplasty needs to be determined. In a very provocative study, Li et al. showed that atorvastatin regulates neointimal growth after pericardial patch angioplasty. This process was associated with infiltration of Ephrin-B2-positive cells, diminished ADAM10 expression, and increased Ephrin-B2 and miR-140 expression. These data show that atorvastatin can play a role in potentially enhancing endothelial repair . Atorvastatin showed a higher number of infiltrating cells and a thicker patch neointima compared with control animals. These data suggest a clinical correlation, that is, patients on lower doses of atorvastatin may have thinner patch neointima, whereas higher doses of atorvastatin may be associated with increased numbers of Ephrin-B2 positive cells and thus may show more arterial-like healing. Mature vascular endothelial cells have a vascular identity of arteries, veins, or lymphatics, and similarly, neointimal endothelial cells also acquire vascular
FIGURE 2.4 Proliferation and macrophage infiltration in the patch neointima on day 7. (a) Immunohistochemistry showing CD68- and PCNA-positive cells in the neointima in the arterioplasty and venoplasty on day 7. (b) Immunofluorescence showing double staining of CD68 and α-actin, CD68 and Ki67, and DAPI in the neointima. Scale bar, 100 μm.
identity depending upon their environment . The Eph-ephrin family of signaling molecules was originally recognized as markers of embryonic vessel identity. Eph receptors and their membrane-associated ligands, ephrins, are now known to have a range of vital functions in vascular physiology. Interactions of Ephs with ephrins at cell-to-cell interfaces promote a variety of cellular responses such as repulsion, adhesion, attraction, and migration, and frequently occur during organ development, including vessel formation . Endothelial cells express Ephrin-B2 and notch-4 but not Eph-B4 and COUP-TFII in arterial neointima, whereas endothelial cells express Eph-B4 and COUP-TFII but not Ephrin-B2 and notch-4 in venous neointima [2,14]. Previously, we showed that venous identity is lost during vein graft adaptation to the arterial environment but arterial markers were not strongly induced in the venous wall . In the rat patch angioplasty model, we showed that autologous tissue patches heal by the acquisition of the vascular identity determined by the environment into which they are implanted, suggesting some plasticity of adult vascular identity . In the polyester patch angioplasty model, cells in the arterial patch were Ephrin-B2- and notch-4-positive, while those in the venous patch were Eph-B4- and COUP-TFII-positive. Venous patches treated with an arteriovenous fistula (AVF) had decreased neointimal thickness. Neointimal endothelial cells expressed Ephrin-B2 and notch-4 in addition to Eph-B4 and COUP-TFII. These data suggest that synthetic patches heal by the acquisition of identity of their environment, similar to tissue patches . These data suggest that endothelial cell identity plays an important role in the patch healing process. Because identity can regulate neointimal hyperplasia, patches coated with arterial or venous endothelial cells may contribute to patch healing or reendothelialization.
2.4 TISSUE-ENGINEERED VASCULAR PATCHES Using advanced techniques of tissue engineering, vascular conduits can be modified or engineered. Tissue-engineered vascular grafts have been showing very promising results in both basic studies as well as clinical trials [12,32,37,38]. We tested several different tissue-engineered patches in the rat patch angioplasty model. We used several different patch materials [5,6] and coated the patches with drugs using hyaluronic acid (HA) solution. HA is a component of the extracellular matrix secreted from both vascular endothelial cells and vascular SMCs that plays crucial roles in cardiovascular physiology . HA can inhibit SMC proliferation and synthetic phenotype change, inhibit platelet activation and aggregation, promote endothelial monolayer repair and functionalization, and prevent inflammation and atherosclerosis . HA can also enhance endothelial cell adhesion, proliferation, migration, and functional factor release . It is clinically used in humans to treat knee osteoarthritis . Another common tool to deliver drugs locally is using nanotechnology. Nanopar ticles (NP) can be made from many materials and can be used to encapsulate many types of therapeutic agents. Poly(lactic-co-glycolic acid) (PLGA) is approved for use in patients and is one of the most effective biodegradable polymeric NP in current use. We previously coated pericardial patches with PLGA NPs that released rapamycin and showed decreased neointimal thickness in the rat venoplasty model .
Biomaterials and Materials for Medicine
Because acute platelet accumulation can induce graft failure, and heparin is widely used clinically, we coated saphenous vein patches with heparin and showed decreased neointima in both the arterioplasty (454 ± 31 μm vs. 157 ± 31 μm) and venoplasty (1,110 ± 177 μm vs. 227 ± 55 μm) models . Heparin-coated grafts and stents are widely used in patients and show good clinical outcomes [41,42], suggesting the use of heparin as a coating for patches, especially in patients prone to thrombosis. The feasibility of composite nanomaterial-tissue patches for vascular and cardiac reconstruction was recently assessed. Porcine vascular tissue was decellularized and conjugated with gold NPs and implanted in bilateral pig carotid arteries. The patches showed regenerating endothelial cell growth and normal healing responses, with excellent integration at 9 weeks. Histology showed cellular ingrowth without immune reactions . This data show the safety of NPs and support their future application in patches. Because there are a large number of neointimal SMC after venoplasty, we conjugated PLGA NP rapamycin to the pericardial patches and implanted them into the IVC. After venoplasty, there were significantly fewer proliferating SMCs and much thinner neointima compared to the control group . These data confirm the utility of NP conjugated to patches. Because macrophages and leukocytes are also found within the neointima [6,31], we determined if manipulation of macrophages and lymphocytes would be another strategy to regulate neointimal formation. As PD-1 is expressed on macrophages and lymphocytes, we conjugated PD-1 to the surface of decellularized rat thoracic artery patches and implanted them into the rat aorta and IVC. In these composite patches, there was a much thinner neointima in the PD-1 treatment groups compared to control groups, with significantly fewer PD-1 (p = 0.0148), CD3 (p = 0.0072), CD68 (p = 0.0001), CD45 (p = 0.001), and PCNA (p